# Electronic Supplementary Material (ESI) for CrystEngComm.
# This journal is © The Royal Society of Chemistry 2014

#######################################################################
#
#                 Cambridge Crystallographic Data Centre
#                                CCDC 
# 
#######################################################################
# 
#  This CIF contains data from an original supplementary publication
#  deposited with the CCDC, and may include chemical, crystal,
#  experimental, refinement, atomic coordinates,
#  anisotropic displacement parameters and molecular geometry data,
#  as required by the journal to which it was submitted.
#
#  This CIF is provided on the understanding that it is used for bona
#  fide research purposes only. It may contain copyright material
#  of the CCDC or of third parties, and may not be copied or further
#  disseminated in any form, whether machine-readable or not,
#  except for the purpose of generating routine backup copies
#  on your local computer system.
# 
#  For further information on the CCDC, data deposition and
#  data retrieval see:
#                         www.ccdc.cam.ac.uk
#
#  Bona fide researchers may freely download Mercury and enCIFer
#  from this site to visualise CIF-encoded structures and 
#  to carry out CIF format checking respectively.
#
data_1

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
;
 ?
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         C30H35K4La3N12O74SiW12
_chemical_formula_sum            'C30 H35 K4 La3 N12 O74 Si W12'
_chemical_formula_weight         4554.91

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
La La -0.2871 2.4523 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           rhombohedral
_symmetry_space_group_name_H-M   R-3
_symmetry_space_group_name_Hall  '-R 3'

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'x+2/3, y+1/3, z+1/3'
'-y+2/3, x-y+1/3, z+1/3'
'-x+y+2/3, -x+1/3, z+1/3'
'x+1/3, y+2/3, z+2/3'
'-y+1/3, x-y+2/3, z+2/3'
'-x+y+1/3, -x+2/3, z+2/3'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'-x+2/3, -y+1/3, -z+1/3'
'y+2/3, -x+y+1/3, -z+1/3'
'x-y+2/3, x+1/3, -z+1/3'
'-x+1/3, -y+2/3, -z+2/3'
'y+1/3, -x+y+2/3, -z+2/3'
'x-y+1/3, x+2/3, -z+2/3'

_cell_length_a                   22.0842(2)
_cell_length_b                   22.0842(2)
_cell_length_c                   28.0921(6)
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_volume                     11865.3(3)
_cell_formula_units_Z            6
_cell_measurement_temperature    296(2)
_cell_measurement_reflns_used    .
_cell_measurement_theta_min      .
_cell_measurement_theta_max      .

_exptl_crystal_description       block
_exptl_crystal_colour            yellow
_exptl_crystal_size_max          0.10
_exptl_crystal_size_mid          0.08
_exptl_crystal_size_min          0.08
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    3.824
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             11902
_exptl_absorpt_coefficient_mu    19.304
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.2484
_exptl_absorpt_correction_T_max  0.3073
_exptl_absorpt_process_details   'SADABS (Sheldrick, 2001)'

_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_detector_area_resol_mean .
_diffrn_standards_number         .
_diffrn_standards_interval_count .
_diffrn_standards_interval_time  .
_diffrn_standards_decay_%        .
_diffrn_reflns_number            16772
_diffrn_reflns_av_R_equivalents  0.0436
_diffrn_reflns_av_sigmaI/netI    0.0390
_diffrn_reflns_limit_h_min       -24
_diffrn_reflns_limit_h_max       21
_diffrn_reflns_limit_k_min       -23
_diffrn_reflns_limit_k_max       24
_diffrn_reflns_limit_l_min       -31
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_theta_min         2.17
_diffrn_reflns_theta_max         23.45
_reflns_number_total             3855
_reflns_number_gt                3219
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       'SMART (Bruker, 2007)'
_computing_cell_refinement       'SMART (Bruker, 2007)'
_computing_data_reduction        'SMART (Bruker, 2007)'
_computing_structure_solution    'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    'SHELXL-97 (Sheldrick, 1997)'
_computing_publication_material  'SHELXL-97 (Sheldrick, 1997)'

_refine_special_details          
;
 Refinement of F² against ALL reflections.  The weighted R-factor wR and
 goodness of fit S are based on F², conventional R-factors R are based
 on F, with F set to zero for negative F². The threshold expression of
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is
 not relevant to the choice of reflections for refinement.  R-factors based
 on F² are statistically about twice as large as those based on F, and R-
 factors based on ALL data will be even larger.
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0330P)²+519.3617P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_number_reflns         3855
_refine_ls_number_parameters     397
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0438
_refine_ls_R_factor_gt           0.0327
_refine_ls_wR_factor_ref         0.0763
_refine_ls_wR_factor_gt          0.0716
_refine_ls_goodness_of_fit_ref   1.011
_refine_ls_restrained_S_all      1.011
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Si Si 0.6667 0.3333 0.1503(2) 0.0100(11) Uani 1 3 d S . .
W1 W 0.71508(2) 0.43470(2) 0.255271(18) 0.01521(14) Uani 1 1 d . . .
W2 W 0.51147(2) 0.33955(2) 0.148829(18) 0.01293(14) Uani 1 1 d . . .
W3 W 0.60949(2) 0.38708(2) 0.049199(18) 0.01647(14) Uani 1 1 d . . .
W4 W 0.66337(2) 0.49074(2) 0.146506(18) 0.01487(14) Uani 1 1 d . . .
La La 0.64247(3) 0.66089(3) 0.19302(3) 0.01468(18) Uani 1 1 d . . .
K1 K 0.24482(19) 0.29378(18) 0.28609(16) 0.0630(11) Uani 1 1 d . . .
O1 O 0.6274(4) 0.3737(4) 0.1306(3) 0.0169(18) Uani 1 1 d . . .
O2 O 0.6667 0.3333 0.2083(5) 0.011(3) Uani 1 3 d S . .
O3 O 0.7477(4) 0.3750(4) 0.2817(3) 0.0208(19) Uani 1 1 d . . .
O4 O 0.7456(4) 0.4990(5) 0.2955(3) 0.027(2) Uani 1 1 d . . .
O5 O 0.6738(4) 0.4677(4) 0.2096(3) 0.0179(19) Uani 1 1 d . . .
O6 O 0.4294(4) 0.3278(4) 0.1551(3) 0.024(2) Uani 1 1 d . . .
O7 O 0.5637(4) 0.4379(4) 0.1575(3) 0.0207(19) Uani 1 1 d . . .
O8 O 0.6750(4) 0.5735(4) 0.1521(3) 0.0192(19) Uani 1 1 d . . .
O9 O 0.6420(4) 0.4761(4) 0.0802(3) 0.0200(19) Uani 1 1 d . . .
O10 O 0.5225(4) 0.3563(4) 0.0809(3) 0.0172(18) Uani 1 1 d . . .
O11 O 0.4921(4) 0.2458(4) 0.1350(3) 0.0192(19) Uani 1 1 d . . .
O12 O 0.5916(4) 0.4065(4) -0.0050(3) 0.032(2) Uani 1 1 d . . .
O13 O 0.5881(4) 0.2936(4) 0.0428(3) 0.0209(19) Uani 1 1 d . . .
O14 O 0.5313(4) 0.3236(4) 0.2105(3) 0.0149(18) Uani 1 1 d . . .
O15 O 0.5324(4) 0.5674(4) 0.1561(3) 0.028(2) Uani 1 1 d . . .
O16 O 0.4329(4) 0.4677(4) 0.1539(3) 0.028(2) Uani 1 1 d . . .
O17 O 0.3570(4) 0.3642(4) 0.2255(3) 0.027(2) Uani 1 1 d . . .
O18 O 0.3969(4) 0.3280(4) 0.2847(3) 0.030(2) Uani 1 1 d . . .
O19 O 0.6776(4) 0.7143(5) 0.2750(3) 0.030(2) Uani 1 1 d . . .
O20 O 0.7503(4) 0.7596(4) 0.3355(3) 0.028(2) Uani 1 1 d . . .
O21 O 0.8672(5) 0.7808(5) 0.3594(3) 0.037(2) Uani 1 1 d . . .
H21 H 0.8282 0.7732 0.3518 0.055 Uiso 1 1 calc R . .
O22 O 0.9405(5) 0.7466(5) 0.3356(4) 0.038(2) Uani 1 1 d . . .
O23 O 0.5373(4) 0.6565(5) 0.2382(4) 0.036(2) Uani 1 1 d . . .
K2 K 0.4443(9) 0.5908(8) 0.1007(6) 0.096(5) Uiso 0.33 1 d P . .
O24 O 0.1761(16) 0.3650(16) 0.2937(11) 0.100(10) Uiso 0.50 1 d P . .
N1 N 0.5730(5) 0.5394(4) 0.2390(3) 0.015(2) Uani 1 1 d . . .
N2 N 0.5232(5) 0.4476(5) 0.2854(4) 0.020(2) Uani 1 1 d . . .
H2 H 0.5179 0.4198 0.3085 0.024 Uiso 1 1 calc R . .
N3 N 0.7491(5) 0.6533(5) 0.2403(4) 0.024(3) Uani 1 1 d . . .
N4 N 0.8494(5) 0.6639(5) 0.2634(4) 0.026(3) Uani 1 1 d . . .
H4 H 0.8853 0.6585 0.2643 0.031 Uiso 1 1 calc R . .
C1 C 0.5813(6) 0.5102(6) 0.2772(5) 0.021(3) Uani 1 1 d . . .
H1 H 0.6213 0.5297 0.2960 0.025 Uiso 1 1 calc R . .
C2 C 0.5064(6) 0.4932(6) 0.2212(4) 0.017(3) Uani 1 1 d . . .
C3 C 0.4739(5) 0.4356(6) 0.2509(4) 0.017(3) Uani 1 1 d . . .
C4 C 0.4885(6) 0.5097(6) 0.1751(5) 0.020(3) Uani 1 1 d . . .
C5 C 0.4038(6) 0.3707(6) 0.2530(5) 0.020(3) Uani 1 1 d . . .
C6 C 0.7968(6) 0.6347(6) 0.2325(5) 0.027(3) Uani 1 1 d . . .
H6 H 0.7938 0.6047 0.2083 0.032 Uiso 1 1 calc R . .
C7 C 0.8358(6) 0.7038(6) 0.2930(5) 0.023(3) Uani 1 1 d . . .
C8 C 0.7741(6) 0.6966(6) 0.2787(5) 0.019(3) Uani 1 1 d . . .
C9 C 0.7309(6) 0.7263(6) 0.2975(5) 0.022(3) Uani 1 1 d . . .
C10 C 0.8865(7) 0.7466(6) 0.3309(5) 0.027(3) Uani 1 1 d . . .
O25 O 0.425(3) 0.714(3) 0.081(2) 0.130(19) Uiso 0.33 1 d P . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Si O1 1.621(8) 2_655 ?
Si O1 1.621(8) 3_665 ?
Si O1 1.621(7) . ?
Si O2 1.630(14) . ?
W1 O4 1.670(9) . ?
W1 O3 1.913(8) 2_655 ?
W1 O5 1.916(7) . ?
W1 O3 1.938(7) . ?
W1 O14 1.942(7) 3_665 ?
W1 O2 2.346(7) . ?
W2 O6 1.707(8) . ?
W2 O14 1.864(8) . ?
W2 O7 1.897(7) . ?
W2 O11 1.933(7) . ?
W2 O10 1.936(8) . ?
W2 O1 2.335(7) . ?
W3 O12 1.681(9) . ?
W3 O13 1.882(7) . ?
W3 O10 1.908(7) . ?
W3 O13 1.914(7) 3_665 ?
W3 O9 1.932(7) . ?
W3 O1 2.365(8) . ?
W3 K1 4.132(3) 15 ?
W4 O8 1.721(7) . ?
W4 O11 1.862(8) 3_665 ?
W4 O5 1.890(8) . ?
W4 O9 1.908(8) . ?
W4 O7 1.932(7) . ?
W4 O1 2.336(7) . ?
W4 K1 3.804(4) 15 ?
La O17 2.458(9) 15 ?
La O16 2.481(8) 15 ?
La O15 2.496(8) . ?
La O19 2.526(9) . ?
La O6 2.589(7) 15 ?
La O23 2.606(8) . ?
La O8 2.637(7) . ?
La N1 2.665(9) . ?
La N3 2.780(10) . ?
La K1 4.406(4) 15 ?
La K2 4.637(17) . ?
K1 O24 2.68(3) . ?
K1 O22 2.693(11) 2_655 ?
K1 O20 2.702(9) 18_545 ?
K1 O9 2.726(8) 14_455 ?
K1 O17 2.757(9) . ?
K1 O18 3.052(10) . ?
K1 O24 3.17(3) 16 ?
K1 O19 3.174(10) 18_545 ?
K1 C5 3.179(12) . ?
K1 C9 3.197(13) 18_545 ?
K1 O8 3.227(9) 14_455 ?
K1 W4 3.804(4) 14_455 ?
O2 W1 2.346(7) 3_665 ?
O2 W1 2.346(7) 2_655 ?
O3 W1 1.913(8) 3_665 ?
O6 La 2.589(7) 14_455 ?
O8 K1 3.227(9) 15 ?
O9 K1 2.727(8) 15 ?
O11 W4 1.862(8) 2_655 ?
O12 K2 2.81(2) 10_665 ?
O13 W3 1.914(7) 2_655 ?
O14 W1 1.942(7) 2_655 ?
O15 C4 1.270(14) . ?
O15 K2 2.734(19) . ?
O16 C4 1.260(14) . ?
O16 La 2.480(8) 14_455 ?
O16 K2 3.001(18) . ?
O17 C5 1.240(14) . ?
O17 La 2.459(9) 14_455 ?
O18 C5 1.251(15) . ?
O19 C9 1.243(15) . ?
O19 K1 3.173(10) 17 ?
O20 C9 1.246(15) . ?
O20 K1 2.702(9) 17 ?
O21 C10 1.310(15) . ?
O22 C10 1.199(15) . ?
O22 K1 2.693(11) 3_665 ?
O23 K2 2.886(18) 15 ?
K2 O12 2.81(2) 10_665 ?
K2 O24 2.84(4) 15 ?
K2 O23 2.886(19) 14_455 ?
K2 O25 3.00(6) . ?
K2 C4 3.21(2) . ?
K2 O25 3.33(6) 3_565 ?
K2 K1 4.250(17) 15 ?
O24 K2 2.84(4) 14_455 ?
O24 K1 3.17(3) 16 ?
N1 C1 1.311(15) . ?
N1 C2 1.398(14) . ?
N2 C1 1.355(14) . ?
N2 C3 1.381(15) . ?
N3 C6 1.326(15) . ?
N3 C8 1.363(16) . ?
N4 C6 1.329(16) . ?
N4 C7 1.351(16) . ?
C2 C3 1.383(16) . ?
C2 C4 1.454(17) . ?
C3 C5 1.495(15) . ?
C7 C8 1.350(16) . ?
C7 C10 1.491(18) . ?
C8 C9 1.498(16) . ?
C9 K1 3.197(13) 17 ?
O25 K2 3.33(6) 2_665 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 Si O1 109.0(3) 2_655 3_665 ?
O1 Si O1 109.0(3) 2_655 . ?
O1 Si O1 109.0(3) 3_665 . ?
O1 Si O2 109.9(3) 2_655 . ?
O1 Si O2 109.9(3) 3_665 . ?
O1 Si O2 109.9(3) . . ?
O4 W1 O3 100.3(4) . 2_655 ?
O4 W1 O5 101.4(4) . . ?
O3 W1 O5 90.5(3) 2_655 . ?
O4 W1 O3 100.9(4) . . ?
O3 W1 O3 88.4(5) 2_655 . ?
O5 W1 O3 157.5(3) . . ?
O4 W1 O14 101.9(4) . 3_665 ?
O3 W1 O14 157.8(3) 2_655 3_665 ?
O5 W1 O14 85.0(3) . 3_665 ?
O3 W1 O14 87.6(3) . 3_665 ?
O4 W1 O2 171.6(4) . . ?
O3 W1 O2 73.8(3) 2_655 . ?
O5 W1 O2 84.8(3) . . ?
O3 W1 O2 73.3(3) . . ?
O14 W1 O2 84.1(3) 3_665 . ?
O6 W2 O14 101.9(4) . . ?
O6 W2 O7 98.8(3) . . ?
O14 W2 O7 91.8(3) . . ?
O6 W2 O11 102.1(3) . . ?
O14 W2 O11 86.0(3) . . ?
O7 W2 O11 159.0(3) . . ?
O6 W2 O10 98.9(4) . . ?
O14 W2 O10 159.0(3) . . ?
O7 W2 O10 87.8(3) . . ?
O11 W2 O10 86.9(3) . . ?
O6 W2 O1 168.8(3) . . ?
O14 W2 O1 86.6(3) . . ?
O7 W2 O1 73.6(3) . . ?
O11 W2 O1 85.5(3) . . ?
O10 W2 O1 73.1(3) . . ?
O12 W3 O13 103.4(4) . . ?
O12 W3 O10 101.0(4) . . ?
O13 W3 O10 89.8(3) . . ?
O12 W3 O13 102.1(4) . 3_665 ?
O13 W3 O13 86.6(4) . 3_665 ?
O10 W3 O13 156.8(3) . 3_665 ?
O12 W3 O9 99.4(4) . . ?
O13 W3 O9 157.1(3) . . ?
O10 W3 O9 87.0(3) . . ?
O13 W3 O9 87.5(3) 3_665 . ?
O12 W3 O1 169.4(3) . . ?
O13 W3 O1 85.5(3) . . ?
O10 W3 O1 72.9(3) . . ?
O13 W3 O1 84.0(3) 3_665 . ?
O9 W3 O1 72.0(3) . . ?
O12 W3 K1 67.9(3) . 15 ?
O13 W3 K1 167.9(2) . 15 ?
O10 W3 K1 83.8(2) . 15 ?
O13 W3 K1 103.3(2) 3_665 15 ?
O9 W3 K1 33.1(2) . 15 ?
O1 W3 K1 102.46(18) . 15 ?
O8 W4 O11 102.9(3) . 3_665 ?
O8 W4 O5 103.2(4) . . ?
O11 W4 O5 87.4(3) 3_665 . ?
O8 W4 O9 99.3(3) . . ?
O11 W4 O9 90.8(3) 3_665 . ?
O5 W4 O9 157.3(3) . . ?
O8 W4 O7 98.5(3) . . ?
O11 W4 O7 158.6(3) 3_665 . ?
O5 W4 O7 86.7(3) . . ?
O9 W4 O7 86.7(3) . . ?
O8 W4 O1 168.5(3) . . ?
O11 W4 O1 86.0(3) 3_665 . ?
O5 W4 O1 84.3(3) . . ?
O9 W4 O1 73.0(3) . . ?
O7 W4 O1 73.0(3) . . ?
O8 W4 K1 57.6(3) . 15 ?
O11 W4 K1 107.4(2) 3_665 15 ?
O5 W4 K1 157.4(2) . 15 ?
O9 W4 K1 42.7(2) . 15 ?
O7 W4 K1 85.0(3) . 15 ?
O1 W4 K1 113.1(2) . 15 ?
O17 La O16 71.1(3) 15 15 ?
O17 La O15 76.8(3) 15 . ?
O16 La O15 101.6(3) 15 . ?
O17 La O19 142.5(3) 15 . ?
O16 La O19 81.6(3) 15 . ?
O15 La O19 135.2(3) . . ?
O17 La O6 70.0(3) 15 15 ?
O16 La O6 74.0(3) 15 15 ?
O15 La O6 146.1(3) . 15 ?
O19 La O6 78.2(3) . 15 ?
O17 La O23 120.0(3) 15 . ?
O16 La O23 67.0(3) 15 . ?
O15 La O23 72.0(3) . . ?
O19 La O23 68.5(3) . . ?
O6 La O23 131.3(3) 15 . ?
O17 La O8 73.0(3) 15 . ?
O16 La O8 143.8(3) 15 . ?
O15 La O8 73.9(3) . . ?
O19 La O8 127.4(3) . . ?
O6 La O8 89.9(2) 15 . ?
O23 La O8 138.6(3) . . ?
O17 La N1 132.3(3) 15 . ?
O16 La N1 137.9(3) 15 . ?
O15 La N1 62.4(3) . . ?
O19 La N1 85.2(3) . . ?
O6 La N1 141.3(3) 15 . ?
O23 La N1 70.9(3) . . ?
O8 La N1 72.8(3) . . ?
O17 La N3 117.3(3) 15 . ?
O16 La N3 127.6(3) 15 . ?
O15 La N3 130.7(3) . . ?
O19 La N3 61.4(3) . . ?
O6 La N3 63.7(3) 15 . ?
O23 La N3 122.1(3) . . ?
O8 La N3 67.4(3) . . ?
N1 La N3 77.7(3) . . ?
O17 La K1 34.51(19) 15 15 ?
O16 La K1 101.3(2) 15 15 ?
O15 La K1 53.3(2) . 15 ?
O19 La K1 170.6(2) . 15 ?
O6 La K1 93.9(2) 15 15 ?
O23 La K1 120.9(2) . 15 ?
O8 La K1 46.65(18) . 15 ?
N1 La K1 98.2(2) . 15 ?
N3 La K1 110.6(2) . 15 ?
O17 La K2 62.5(3) 15 . ?
O16 La K2 73.2(3) 15 . ?
O15 La K2 28.9(3) . . ?
O19 La K2 133.2(3) . . ?
O6 La K2 128.6(3) 15 . ?
O23 La K2 65.5(3) . . ?
O8 La K2 93.9(3) . . ?
N1 La K2 87.9(3) . . ?
N3 La K2 159.0(3) . . ?
K1 La K2 56.0(2) 15 . ?
O24 K1 O22 136.9(7) . 2_655 ?
O24 K1 O20 69.1(7) . 18_545 ?
O22 K1 O20 107.9(3) 2_655 18_545 ?
O24 K1 O9 101.9(7) . 14_455 ?
O22 K1 O9 72.4(3) 2_655 14_455 ?
O20 K1 O9 167.7(3) 18_545 14_455 ?
O24 K1 O17 109.3(7) . . ?
O22 K1 O17 111.7(3) 2_655 . ?
O20 K1 O17 77.0(3) 18_545 . ?
O9 K1 O17 114.6(3) 14_455 . ?
O24 K1 O18 136.9(7) . . ?
O22 K1 O18 71.9(3) 2_655 . ?
O20 K1 O18 71.2(3) 18_545 . ?
O9 K1 O18 119.5(3) 14_455 . ?
O17 K1 O18 44.4(2) . . ?
O24 K1 O24 50.8(11) . 16 ?
O22 K1 O24 86.7(6) 2_655 16 ?
O20 K1 O24 71.9(6) 18_545 16 ?
O9 K1 O24 95.9(6) 14_455 16 ?
O17 K1 O24 147.6(6) . 16 ?
O18 K1 O24 128.5(6) . 16 ?
O24 K1 O19 86.0(7) . 18_545 ?
O22 K1 O19 69.2(3) 2_655 18_545 ?
O20 K1 O19 43.2(3) 18_545 18_545 ?
O9 K1 O19 130.2(3) 14_455 18_545 ?
O17 K1 O19 108.3(3) . 18_545 ?
O18 K1 O19 76.5(3) . 18_545 ?
O24 K1 O19 52.0(6) 16 18_545 ?
O24 K1 C5 120.4(7) . . ?
O22 K1 C5 94.5(3) 2_655 . ?
O20 K1 C5 67.2(3) 18_545 . ?
O9 K1 C5 125.1(3) 14_455 . ?
O17 K1 C5 22.7(3) . . ?
O18 K1 C5 23.0(3) . . ?
O24 K1 C5 137.4(6) 16 . ?
O19 K1 C5 88.7(3) 18_545 . ?
O24 K1 C9 82.6(7) . 18_545 ?
O22 K1 C9 85.8(3) 2_655 18_545 ?
O20 K1 C9 22.4(3) 18_545 18_545 ?
O9 K1 C9 152.7(3) 14_455 18_545 ?
O17 K1 C9 88.4(3) . 18_545 ?
O18 K1 C9 66.3(3) . 18_545 ?
O24 K1 C9 65.8(6) 16 18_545 ?
O19 K1 C9 22.5(3) 18_545 18_545 ?
C5 K1 C9 71.8(3) . 18_545 ?
O24 K1 O8 114.4(7) . 14_455 ?
O22 K1 O8 97.1(3) 2_655 14_455 ?
O20 K1 O8 136.2(3) 18_545 14_455 ?
O9 K1 O8 54.6(2) 14_455 14_455 ?
O17 K1 O8 60.3(2) . 14_455 ?
O18 K1 O8 83.7(2) . 14_455 ?
O24 K1 O8 146.5(6) 16 14_455 ?
O19 K1 O8 158.6(3) 18_545 14_455 ?
C5 K1 O8 75.7(3) . 14_455 ?
C9 K1 O8 147.4(3) 18_545 14_455 ?
O24 K1 W4 107.1(7) . 14_455 ?
O22 K1 W4 87.8(2) 2_655 14_455 ?
O20 K1 W4 160.8(3) 18_545 14_455 ?
O9 K1 W4 28.31(17) 14_455 14_455 ?
O17 K1 W4 87.1(2) . 14_455 ?
O18 K1 W4 104.6(2) . 14_455 ?
O24 K1 W4 121.2(6) 16 14_455 ?
O19 K1 W4 155.7(2) 18_545 14_455 ?
C5 K1 W4 101.4(2) . 14_455 ?
C9 K1 W4 170.2(2) 18_545 14_455 ?
O8 K1 W4 26.76(13) 14_455 14_455 ?
Si O1 W2 123.3(4) . . ?
Si O1 W4 124.3(4) . . ?
W2 O1 W4 91.6(3) . . ?
Si O1 W3 124.6(4) . . ?
W2 O1 W3 91.6(3) . . ?
W4 O1 W3 91.8(3) . . ?
Si O2 W1 124.2(3) . 3_665 ?
Si O2 W1 124.2(3) . . ?
W1 O2 W1 91.5(4) 3_665 . ?
Si O2 W1 124.2(3) . 2_655 ?
W1 O2 W1 91.5(4) 3_665 2_655 ?
W1 O2 W1 91.5(4) . 2_655 ?
W1 O3 W1 121.4(4) 3_665 . ?
W4 O5 W1 151.1(4) . . ?
W2 O6 La 156.5(4) . 14_455 ?
W2 O7 W4 121.9(4) . . ?
W4 O8 La 150.0(4) . . ?
W4 O8 K1 95.6(3) . 15 ?
La O8 K1 96.9(2) . 15 ?
W4 O9 W3 123.2(4) . . ?
W4 O9 K1 109.0(3) . 15 ?
W3 O9 K1 124.1(4) . 15 ?
W3 O10 W2 122.4(4) . . ?
W4 O11 W2 149.6(4) 2_655 . ?
W3 O12 K2 167.3(6) . 10_665 ?
W3 O13 W3 150.9(4) . 2_655 ?
W2 O14 W1 151.7(4) . 2_655 ?
C4 O15 La 126.4(8) . . ?
C4 O15 K2 99.9(8) . . ?
La O15 K2 124.9(5) . . ?
C4 O16 La 154.1(8) . 14_455 ?
C4 O16 K2 87.6(7) . . ?
La O16 K2 118.0(4) 14_455 . ?
C5 O17 La 141.2(8) . 14_455 ?
C5 O17 K1 98.1(7) . . ?
La O17 K1 115.2(3) 14_455 . ?
C5 O18 K1 84.2(7) . . ?
C9 O19 La 126.9(8) . . ?
C9 O19 K1 79.8(7) . 17 ?
La O19 K1 146.0(3) . 17 ?
C9 O20 K1 101.7(7) . 17 ?
C10 O22 K1 142.4(9) . 3_665 ?
La O23 K2 117.8(5) . 15 ?
O15 K2 O12 141.5(7) . 10_665 ?
O15 K2 O24 77.8(8) . 15 ?
O12 K2 O24 66.5(8) 10_665 15 ?
O15 K2 O23 101.7(6) . 14_455 ?
O12 K2 O23 81.3(5) 10_665 14_455 ?
O24 K2 O23 72.2(8) 15 14_455 ?
O15 K2 O25 135.4(13) . . ?
O12 K2 O25 68.5(12) 10_665 . ?
O24 K2 O25 131.1(15) 15 . ?
O23 K2 O25 118.2(12) 14_455 . ?
O15 K2 O16 44.9(3) . . ?
O12 K2 O16 126.8(6) 10_665 . ?
O24 K2 O16 70.0(8) 15 . ?
O23 K2 O16 57.0(4) 14_455 . ?
O25 K2 O16 158.0(13) . . ?
O15 K2 C4 23.0(3) . . ?
O12 K2 C4 143.4(7) 10_665 . ?
O24 K2 C4 78.0(8) 15 . ?
O23 K2 C4 79.9(5) 14_455 . ?
O25 K2 C4 147.9(13) . . ?
O16 K2 C4 23.1(3) . . ?
O15 K2 O25 150.7(12) . 3_565 ?
O12 K2 O25 63.4(11) 10_665 3_565 ?
O24 K2 O25 114.4(13) 15 3_565 ?
O23 K2 O25 61.0(10) 14_455 3_565 ?
O25 K2 O25 57(2) . 3_565 ?
O16 K2 O25 111.9(11) . 3_565 ?
C4 K2 O25 129.7(12) . 3_565 ?
O15 K2 K1 55.9(3) . 15 ?
O12 K2 K1 86.4(4) 10_665 15 ?
O24 K2 K1 38.4(7) 15 15 ?
O23 K2 K1 107.5(5) 14_455 15 ?
O25 K2 K1 122.0(12) . 15 ?
O16 K2 K1 77.7(4) . 15 ?
C4 K2 K1 70.0(4) . 15 ?
O25 K2 K1 148.3(12) 3_565 15 ?
O15 K2 La 26.2(2) . . ?
O12 K2 La 139.2(5) 10_665 . ?
O24 K2 La 92.8(7) 15 . ?
O23 K2 La 127.2(5) 14_455 . ?
O25 K2 La 109.7(12) . . ?
O16 K2 La 70.2(4) . . ?
C4 K2 La 47.3(3) . . ?
O25 K2 La 152.1(12) 3_565 . ?
K1 K2 La 59.2(2) 15 . ?
K1 O24 K2 100.7(10) . 14_455 ?
K1 O24 K1 129.2(11) . 16 ?
K2 O24 K1 123.1(11) 14_455 16 ?
C1 N1 C2 106.7(9) . . ?
C1 N1 La 137.7(7) . . ?
C2 N1 La 115.4(7) . . ?
C1 N2 C3 109.2(10) . . ?
C6 N3 C8 103.9(10) . . ?
C6 N3 La 140.2(9) . . ?
C8 N3 La 113.3(7) . . ?
C6 N4 C7 107.0(10) . . ?
N1 C1 N2 110.3(10) . . ?
C3 C2 N1 109.2(10) . . ?
C3 C2 C4 133.4(11) . . ?
N1 C2 C4 116.9(10) . . ?
N2 C3 C2 104.5(9) . . ?
N2 C3 C5 119.7(10) . . ?
C2 C3 C5 135.9(11) . . ?
O16 C4 O15 121.0(12) . . ?
O16 C4 C2 121.5(11) . . ?
O15 C4 C2 117.4(10) . . ?
O16 C4 K2 69.3(7) . . ?
O15 C4 K2 57.2(7) . . ?
C2 C4 K2 156.7(8) . . ?
O17 C5 O18 125.2(11) . . ?
O17 C5 C3 119.3(11) . . ?
O18 C5 C3 115.4(11) . . ?
O17 C5 K1 59.2(6) . . ?
O18 C5 K1 72.8(6) . . ?
C3 C5 K1 149.5(8) . . ?
N3 C6 N4 112.3(11) . . ?
C8 C7 N4 106.2(11) . . ?
C8 C7 C10 133.0(12) . . ?
N4 C7 C10 120.7(10) . . ?
C7 C8 N3 110.5(11) . . ?
C7 C8 C9 131.9(12) . . ?
N3 C8 C9 117.5(11) . . ?
O19 C9 O20 124.8(11) . . ?
O19 C9 C8 118.1(12) . . ?
O20 C9 C8 117.1(11) . . ?
O19 C9 K1 77.7(7) . 17 ?
O20 C9 K1 55.9(6) . 17 ?
C8 C9 K1 144.6(8) . 17 ?
O22 C10 O21 122.9(13) . . ?
O22 C10 C7 120.8(12) . . ?
O21 C10 C7 116.3(11) . . ?
K2 O25 K2 159(2) . 2_665 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O1 Si O1 W2 61.7(8) 2_655 . . . ?
O1 Si O1 W2 -179.4(3) 3_665 . . . ?
O2 Si O1 W2 -58.8(5) . . . . ?
O1 Si O1 W4 -179.0(3) 2_655 . . . ?
O1 Si O1 W4 -60.1(8) 3_665 . . . ?
O2 Si O1 W4 60.4(5) . . . . ?
O1 Si O1 W3 -57.8(5) 2_655 . . . ?
O1 Si O1 W3 61.0(5) 3_665 . . . ?
O2 Si O1 W3 -178.4(3) . . . . ?
O6 W2 O1 Si -178.4(16) . . . . ?
O14 W2 O1 Si 40.9(5) . . . . ?
O7 W2 O1 Si 133.8(6) . . . . ?
O11 W2 O1 Si -45.3(5) . . . . ?
O10 W2 O1 Si -133.5(6) . . . . ?
O6 W2 O1 W4 47.7(18) . . . . ?
O14 W2 O1 W4 -93.0(3) . . . . ?
O7 W2 O1 W4 -0.1(3) . . . . ?
O11 W2 O1 W4 -179.2(3) . . . . ?
O10 W2 O1 W4 92.7(3) . . . . ?
O6 W2 O1 W3 -44.2(18) . . . . ?
O14 W2 O1 W3 175.2(3) . . . . ?
O7 W2 O1 W3 -92.0(3) . . . . ?
O11 W2 O1 W3 88.9(3) . . . . ?
O10 W2 O1 W3 0.8(3) . . . . ?
O8 W4 O1 Si -176.1(14) . . . . ?
O11 W4 O1 Si 43.0(5) 3_665 . . . ?
O5 W4 O1 Si -44.8(5) . . . . ?
O9 W4 O1 Si 135.1(6) . . . . ?
O7 W4 O1 Si -133.1(6) . . . . ?
K1 W4 O1 Si 150.2(4) 15 . . . ?
O8 W4 O1 W2 -42.9(17) . . . . ?
O11 W4 O1 W2 176.2(3) 3_665 . . . ?
O5 W4 O1 W2 88.4(3) . . . . ?
O9 W4 O1 W2 -91.7(3) . . . . ?
O7 W4 O1 W2 0.1(3) . . . . ?
K1 W4 O1 W2 -76.7(2) 15 . . . ?
O8 W4 O1 W3 48.8(17) . . . . ?
O11 W4 O1 W3 -92.2(3) 3_665 . . . ?
O5 W4 O1 W3 180.0(3) . . . . ?
O9 W4 O1 W3 -0.1(3) . . . . ?
O7 W4 O1 W3 91.7(3) . . . . ?
K1 W4 O1 W3 15.0(3) 15 . . . ?
O12 W3 O1 Si -171.7(17) . . . . ?
O13 W3 O1 Si 41.4(5) . . . . ?
O10 W3 O1 Si 132.6(5) . . . . ?
O13 W3 O1 Si -45.7(5) 3_665 . . . ?
O9 W3 O1 Si -134.9(5) . . . . ?
K1 W3 O1 Si -148.0(4) 15 . . . ?
O12 W3 O1 W2 54.9(19) . . . . ?
O13 W3 O1 W2 -92.0(3) . . . . ?
O10 W3 O1 W2 -0.8(3) . . . . ?
O13 W3 O1 W2 -179.0(3) 3_665 . . . ?
O9 W3 O1 W2 91.7(3) . . . . ?
K1 W3 O1 W2 78.7(2) 15 . . . ?
O12 W3 O1 W4 -36.7(19) . . . . ?
O13 W3 O1 W4 176.4(3) . . . . ?
O10 W3 O1 W4 -92.4(3) . . . . ?
O13 W3 O1 W4 89.3(3) 3_665 . . . ?
O9 W3 O1 W4 0.1(3) . . . . ?
K1 W3 O1 W4 -13.0(2) 15 . . . ?
O1 Si O2 W1 61.9(3) 2_655 . . 3_665 ?
O1 Si O2 W1 -58.1(3) 3_665 . . 3_665 ?
O1 Si O2 W1 -178.1(3) . . . 3_665 ?
O1 Si O2 W1 -178.1(3) 2_655 . . . ?
O1 Si O2 W1 61.9(3) 3_665 . . . ?
O1 Si O2 W1 -58.1(3) . . . . ?
O1 Si O2 W1 -58.1(3) 2_655 . . 2_655 ?
O1 Si O2 W1 -178.1(3) 3_665 . . 2_655 ?
O1 Si O2 W1 61.9(3) . . . 2_655 ?
O4 W1 O2 Si 179(100) . . . . ?
O3 W1 O2 Si 133.4(2) 2_655 . . . ?
O5 W1 O2 Si 41.3(2) . . . . ?
O3 W1 O2 Si -133.4(2) . . . . ?
O14 W1 O2 Si -44.2(2) 3_665 . . . ?
O4 W1 O2 W1 -46.6(19) . . . 3_665 ?
O3 W1 O2 W1 -92.4(4) 2_655 . . 3_665 ?
O5 W1 O2 W1 175.6(3) . . . 3_665 ?
O3 W1 O2 W1 0.9(3) . . . 3_665 ?
O14 W1 O2 W1 90.1(3) 3_665 . . 3_665 ?
O4 W1 O2 W1 44.9(19) . . . 2_655 ?
O3 W1 O2 W1 -0.9(3) 2_655 . . 2_655 ?
O5 W1 O2 W1 -93.0(3) . . . 2_655 ?
O3 W1 O2 W1 92.4(3) . . . 2_655 ?
O14 W1 O2 W1 -178.4(3) 3_665 . . 2_655 ?
O4 W1 O3 W1 172.5(5) . . . 3_665 ?
O3 W1 O3 W1 72.2(5) 2_655 . . 3_665 ?
O5 W1 O3 W1 -15.3(11) . . . 3_665 ?
O14 W1 O3 W1 -85.9(5) 3_665 . . 3_665 ?
O2 W1 O3 W1 -1.3(4) . . . 3_665 ?
O8 W4 O5 W1 -129.1(9) . . . . ?
O11 W4 O5 W1 -26.4(9) 3_665 . . . ?
O9 W4 O5 W1 59.6(14) . . . . ?
O7 W4 O5 W1 132.9(9) . . . . ?
O1 W4 O5 W1 59.8(9) . . . . ?
K1 W4 O5 W1 -158.5(5) 15 . . . ?
O4 W1 O5 W4 127.0(9) . . . . ?
O3 W1 O5 W4 -132.4(9) 2_655 . . . ?
O3 W1 O5 W4 -45.3(14) . . . . ?
O14 W1 O5 W4 25.8(9) 3_665 . . . ?
O2 W1 O5 W4 -58.7(9) . . . . ?
O14 W2 O6 La 142.5(11) . . . 14_455 ?
O7 W2 O6 La 48.7(12) . . . 14_455 ?
O11 W2 O6 La -129.1(11) . . . 14_455 ?
O10 W2 O6 La -40.4(12) . . . 14_455 ?
O1 W2 O6 La 3(3) . . . 14_455 ?
O6 W2 O7 W4 -171.6(5) . . . . ?
O14 W2 O7 W4 86.1(5) . . . . ?
O11 W2 O7 W4 2.5(13) . . . . ?
O10 W2 O7 W4 -72.9(5) . . . . ?
O1 W2 O7 W4 0.1(4) . . . . ?
O8 W4 O7 W2 172.0(5) . . . . ?
O11 W4 O7 W2 -10.8(13) 3_665 . . . ?
O5 W4 O7 W2 -85.2(5) . . . . ?
O9 W4 O7 W2 73.1(5) . . . . ?
O1 W4 O7 W2 -0.1(4) . . . . ?
K1 W4 O7 W2 115.9(5) 15 . . . ?
O11 W4 O8 La -143.1(8) 3_665 . . . ?
O5 W4 O8 La -52.7(9) . . . . ?
O9 W4 O8 La 123.9(8) . . . . ?
O7 W4 O8 La 35.9(9) . . . . ?
O1 W4 O8 La 77(2) . . . . ?
K1 W4 O8 La 114.4(9) 15 . . . ?
O11 W4 O8 K1 102.5(3) 3_665 . . 15 ?
O5 W4 O8 K1 -167.1(3) . . . 15 ?
O9 W4 O8 K1 9.6(3) . . . 15 ?
O7 W4 O8 K1 -78.5(3) . . . 15 ?
O1 W4 O8 K1 -37.3(17) . . . 15 ?
O17 La O8 W4 -140.4(9) 15 . . . ?
O16 La O8 W4 -147.4(7) 15 . . . ?
O15 La O8 W4 -59.7(8) . . . . ?
O19 La O8 W4 75.5(9) . . . . ?
O6 La O8 W4 150.5(8) 15 . . . ?
O23 La O8 W4 -24.1(10) . . . . ?
N1 La O8 W4 5.8(8) . . . . ?
N3 La O8 W4 89.2(9) . . . . ?
K1 La O8 W4 -114.1(9) 15 . . . ?
K2 La O8 W4 -80.8(8) . . . . ?
O17 La O8 K1 -26.3(3) 15 . . 15 ?
O16 La O8 K1 -33.4(5) 15 . . 15 ?
O15 La O8 K1 54.4(3) . . . 15 ?
O19 La O8 K1 -170.4(3) . . . 15 ?
O6 La O8 K1 -95.4(3) 15 . . 15 ?
O23 La O8 K1 89.9(4) . . . 15 ?
N1 La O8 K1 119.8(3) . . . 15 ?
N3 La O8 K1 -156.7(3) . . . 15 ?
K2 La O8 K1 33.3(3) . . . 15 ?
O8 W4 O9 W3 -171.2(5) . . . . ?
O11 W4 O9 W3 85.6(5) 3_665 . . . ?
O5 W4 O9 W3 0.3(11) . . . . ?
O7 W4 O9 W3 -73.1(5) . . . . ?
O1 W4 O9 W3 0.1(4) . . . . ?
K1 W4 O9 W3 -159.2(7) 15 . . . ?
O8 W4 O9 K1 -11.9(4) . . . 15 ?
O11 W4 O9 K1 -115.1(3) 3_665 . . 15 ?
O5 W4 O9 K1 159.5(7) . . . 15 ?
O7 W4 O9 K1 86.2(3) . . . 15 ?
O1 W4 O9 K1 159.3(4) . . . 15 ?
O12 W3 O9 W4 173.4(5) . . . . ?
O13 W3 O9 W4 -9.7(11) . . . . ?
O10 W3 O9 W4 72.8(5) . . . . ?
O13 W3 O9 W4 -84.7(5) 3_665 . . . ?
O1 W3 O9 W4 -0.1(4) . . . . ?
K1 W3 O9 W4 156.1(8) 15 . . . ?
O12 W3 O9 K1 17.4(5) . . . 15 ?
O13 W3 O9 K1 -165.8(6) . . . 15 ?
O10 W3 O9 K1 -83.3(4) . . . 15 ?
O13 W3 O9 K1 119.2(5) 3_665 . . 15 ?
O1 W3 O9 K1 -156.2(5) . . . 15 ?
O12 W3 O10 W2 -169.9(5) . . . . ?
O13 W3 O10 W2 86.4(5) . . . . ?
O13 W3 O10 W2 5.5(11) 3_665 . . . ?
O9 W3 O10 W2 -70.9(5) . . . . ?
O1 W3 O10 W2 1.1(4) . . . . ?
K1 W3 O10 W2 -104.0(4) 15 . . . ?
O6 W2 O10 W3 170.9(4) . . . . ?
O14 W2 O10 W3 -17.0(11) . . . . ?
O7 W2 O10 W3 72.3(5) . . . . ?
O11 W2 O10 W3 -87.4(5) . . . . ?
O1 W2 O10 W3 -1.1(4) . . . . ?
O6 W2 O11 W4 -132.0(9) . . . 2_655 ?
O14 W2 O11 W4 -30.6(9) . . . 2_655 ?
O7 W2 O11 W4 54.0(15) . . . 2_655 ?
O10 W2 O11 W4 129.6(9) . . . 2_655 ?
O1 W2 O11 W4 56.3(9) . . . 2_655 ?
O13 W3 O12 K2 -4(3) . . . 10_665 ?
O10 W3 O12 K2 -96(3) . . . 10_665 ?
O13 W3 O12 K2 85(3) 3_665 . . 10_665 ?
O9 W3 O12 K2 175(3) . . . 10_665 ?
O1 W3 O12 K2 -150(2) . . . 10_665 ?
K1 W3 O12 K2 -175(3) 15 . . 10_665 ?
O12 W3 O13 W3 128.1(10) . . . 2_655 ?
O10 W3 O13 W3 -130.7(10) . . . 2_655 ?
O13 W3 O13 W3 26.4(12) 3_665 . . 2_655 ?
O9 W3 O13 W3 -48.7(15) . . . 2_655 ?
O1 W3 O13 W3 -57.8(10) . . . 2_655 ?
K1 W3 O13 W3 170.9(4) 15 . . 2_655 ?
O6 W2 O14 W1 133.3(9) . . . 2_655 ?
O7 W2 O14 W1 -127.4(9) . . . 2_655 ?
O11 W2 O14 W1 31.8(9) . . . 2_655 ?
O10 W2 O14 W1 -38.8(15) . . . 2_655 ?
O1 W2 O14 W1 -53.9(9) . . . 2_655 ?
O17 La O15 C4 163.1(10) 15 . . . ?
O16 La O15 C4 -129.7(9) 15 . . . ?
O19 La O15 C4 -40.0(11) . . . . ?
O6 La O15 C4 151.7(8) 15 . . . ?
O23 La O15 C4 -68.8(9) . . . . ?
O8 La O15 C4 87.3(9) . . . . ?
N1 La O15 C4 8.6(9) . . . . ?
N3 La O15 C4 48.3(11) . . . . ?
K1 La O15 C4 134.8(10) 15 . . . ?
K2 La O15 C4 -140.7(13) . . . . ?
O17 La O15 K2 -56.2(6) 15 . . . ?
O16 La O15 K2 10.9(6) 15 . . . ?
O19 La O15 K2 100.7(6) . . . . ?
O6 La O15 K2 -67.6(8) 15 . . . ?
O23 La O15 K2 71.8(6) . . . . ?
O8 La O15 K2 -132.0(6) . . . . ?
N1 La O15 K2 149.2(7) . . . . ?
N3 La O15 K2 -171.0(6) . . . . ?
K1 La O15 K2 -84.6(6) 15 . . . ?
O24 K1 O17 C5 123.6(10) . . . . ?
O22 K1 O17 C5 -42.8(8) 2_655 . . . ?
O20 K1 O17 C5 61.5(7) 18_545 . . . ?
O9 K1 O17 C5 -122.7(7) 14_455 . . . ?
O18 K1 O17 C5 -14.9(7) . . . . ?
O24 K1 O17 C5 78.0(14) 16 . . . ?
O19 K1 O17 C5 31.4(8) 18_545 . . . ?
C9 K1 O17 C5 42.0(7) 18_545 . . . ?
O8 K1 O17 C5 -128.6(8) 14_455 . . . ?
W4 K1 O17 C5 -129.3(7) 14_455 . . . ?
O24 K1 O17 La -77.0(8) . . . 14_455 ?
O22 K1 O17 La 116.6(4) 2_655 . . 14_455 ?
O20 K1 O17 La -139.0(4) 18_545 . . 14_455 ?
O9 K1 O17 La 36.7(5) 14_455 . . 14_455 ?
O18 K1 O17 La 144.6(5) . . . 14_455 ?
O24 K1 O17 La -122.6(11) 16 . . 14_455 ?
O19 K1 O17 La -169.1(3) 18_545 . . 14_455 ?
C5 K1 O17 La 159.4(9) . . . 14_455 ?
C9 K1 O17 La -158.6(4) 18_545 . . 14_455 ?
O8 K1 O17 La 30.8(3) 14_455 . . 14_455 ?
W4 K1 O17 La 30.1(3) 14_455 . . 14_455 ?
O24 K1 O18 C5 -51.7(13) . . . . ?
O22 K1 O18 C5 167.4(8) 2_655 . . . ?
O20 K1 O18 C5 -75.7(7) 18_545 . . . ?
O9 K1 O18 C5 110.8(7) 14_455 . . . ?
O17 K1 O18 C5 14.7(7) . . . . ?
O24 K1 O18 C5 -122.3(10) 16 . . . ?
O19 K1 O18 C5 -120.4(7) 18_545 . . . ?
C9 K1 O18 C5 -99.2(7) 18_545 . . . ?
O8 K1 O18 C5 67.8(7) 14_455 . . . ?
W4 K1 O18 C5 84.6(7) 14_455 . . . ?
O17 La O19 C9 -85.2(11) 15 . . . ?
O16 La O19 C9 -128.2(10) 15 . . . ?
O15 La O19 C9 133.7(9) . . . . ?
O6 La O19 C9 -53.0(10) 15 . . . ?
O23 La O19 C9 163.2(10) . . . . ?
O8 La O19 C9 27.7(11) . . . . ?
N1 La O19 C9 91.8(10) . . . . ?
N3 La O19 C9 13.3(9) . . . . ?
K1 La O19 C9 -20(2) 15 . . . ?
K2 La O19 C9 174.4(9) . . . . ?
O17 La O19 K1 139.1(6) 15 . . 17 ?
O16 La O19 K1 96.0(6) 15 . . 17 ?
O15 La O19 K1 -2.1(8) . . . 17 ?
O6 La O19 K1 171.3(6) 15 . . 17 ?
O23 La O19 K1 27.5(6) . . . 17 ?
O8 La O19 K1 -108.0(6) . . . 17 ?
N1 La O19 K1 -43.9(6) . . . 17 ?
N3 La O19 K1 -122.5(7) . . . 17 ?
K1 La O19 K1 -155.6(8) 15 . . 17 ?
K2 La O19 K1 38.6(8) . . . 17 ?
O17 La O23 K2 -53.4(6) 15 . . 15 ?
O16 La O23 K2 -4.0(5) 15 . . 15 ?
O15 La O23 K2 -115.6(6) . . . 15 ?
O19 La O23 K2 85.8(6) . . . 15 ?
O6 La O23 K2 35.5(7) 15 . . 15 ?
O8 La O23 K2 -151.6(5) . . . 15 ?
N1 La O23 K2 178.2(6) . . . 15 ?
N3 La O23 K2 117.1(5) . . . 15 ?
K1 La O23 K2 -93.6(5) 15 . . 15 ?
K2 La O23 K2 -85.3(6) . . . 15 ?
C4 O15 K2 O12 -109.8(12) . . . 10_665 ?
La O15 K2 O12 101.4(11) . . . 10_665 ?
C4 O15 K2 O24 -87.9(10) . . . 15 ?
La O15 K2 O24 123.3(8) . . . 15 ?
C4 O15 K2 O23 -19.2(9) . . . 14_455 ?
La O15 K2 O23 -168.0(4) . . . 14_455 ?
C4 O15 K2 O25 134.4(19) . . . . ?
La O15 K2 O25 -14(2) . . . . ?
C4 O15 K2 O16 -14.1(7) . . . . ?
La O15 K2 O16 -162.9(7) . . . . ?
La O15 K2 C4 -148.8(10) . . . . ?
C4 O15 K2 O25 31(3) . . . 3_565 ?
La O15 K2 O25 -118(2) . . . 3_565 ?
C4 O15 K2 K1 -122.5(8) . . . 15 ?
La O15 K2 K1 88.7(5) . . . 15 ?
C4 O15 K2 La 148.8(10) . . . . ?
C4 O16 K2 O15 14.0(7) . . . . ?
La O16 K2 O15 -170.3(6) 14_455 . . . ?
C4 O16 K2 O12 143.4(9) . . . 10_665 ?
La O16 K2 O12 -40.9(9) 14_455 . . 10_665 ?
C4 O16 K2 O24 106.7(10) . . . 15 ?
La O16 K2 O24 -77.5(8) 14_455 . . 15 ?
C4 O16 K2 O23 -171.9(8) . . . 14_455 ?
La O16 K2 O23 3.8(5) 14_455 . . 14_455 ?
C4 O16 K2 O25 -88(3) . . . . ?
La O16 K2 O25 88(3) 14_455 . . . ?
La O16 K2 C4 175.7(10) 14_455 . . . ?
C4 O16 K2 O25 -144.1(14) . . . 3_565 ?
La O16 K2 O25 31.6(13) 14_455 . . 3_565 ?
C4 O16 K2 K1 67.5(7) . . . 15 ?
La O16 K2 K1 -116.7(4) 14_455 . . 15 ?
C4 O16 K2 La 6.1(7) . . . . ?
La O16 K2 La -178.2(4) 14_455 . . . ?
O17 La K2 O15 114.2(6) 15 . . . ?
O16 La K2 O15 -168.8(7) 15 . . . ?
O19 La K2 O15 -108.3(6) . . . . ?
O6 La K2 O15 138.7(6) 15 . . . ?
O23 La K2 O15 -96.9(6) . . . . ?
O8 La K2 O15 45.7(6) . . . . ?
N1 La K2 O15 -27.0(6) . . . . ?
N3 La K2 O15 19.2(12) . . . . ?
K1 La K2 O15 74.5(6) 15 . . . ?
O17 La K2 O12 3.0(7) 15 . . 10_665 ?
O16 La K2 O12 80.0(8) 15 . . 10_665 ?
O15 La K2 O12 -111.1(11) . . . 10_665 ?
O19 La K2 O12 140.5(7) . . . 10_665 ?
O6 La K2 O12 27.6(10) 15 . . 10_665 ?
O23 La K2 O12 151.9(9) . . . 10_665 ?
O8 La K2 O12 -65.5(8) . . . 10_665 ?
N1 La K2 O12 -138.1(8) . . . 10_665 ?
N3 La K2 O12 -91.9(11) . . . 10_665 ?
K1 La K2 O12 -36.7(7) 15 . . 10_665 ?
O17 La K2 O24 59.3(7) 15 . . 15 ?
O16 La K2 O24 136.3(8) 15 . . 15 ?
O15 La K2 O24 -54.9(8) . . . 15 ?
O19 La K2 O24 -163.2(7) . . . 15 ?
O6 La K2 O24 83.9(8) 15 . . 15 ?
O23 La K2 O24 -151.8(8) . . . 15 ?
O8 La K2 O24 -9.2(8) . . . 15 ?
N1 La K2 O24 -81.9(8) . . . 15 ?
N3 La K2 O24 -35.7(12) . . . 15 ?
K1 La K2 O24 19.6(7) 15 . . 15 ?
O17 La K2 O23 129.0(7) 15 . . 14_455 ?
O16 La K2 O23 -154.0(7) 15 . . 14_455 ?
O15 La K2 O23 14.8(6) . . . 14_455 ?
O19 La K2 O23 -93.5(7) . . . 14_455 ?
O6 La K2 O23 153.6(5) 15 . . 14_455 ?
O23 La K2 O23 -82.1(7) . . . 14_455 ?
O8 La K2 O23 60.5(7) . . . 14_455 ?
N1 La K2 O23 -12.1(7) . . . 14_455 ?
N3 La K2 O23 34.0(13) . . . 14_455 ?
K1 La K2 O23 89.3(6) 15 . . 14_455 ?
O17 La K2 O25 -76.5(13) 15 . . . ?
O16 La K2 O25 0.5(13) 15 . . . ?
O15 La K2 O25 169.3(15) . . . . ?
O19 La K2 O25 61.0(14) . . . . ?
O6 La K2 O25 -51.9(14) 15 . . . ?
O23 La K2 O25 72.4(13) . . . . ?
O8 La K2 O25 -145.0(13) . . . . ?
N1 La K2 O25 142.3(13) . . . . ?
N3 La K2 O25 -171.5(14) . . . . ?
K1 La K2 O25 -116.2(13) 15 . . . ?
O17 La K2 O16 126.9(4) 15 . . . ?
O16 La K2 O16 -156.1(4) 15 . . . ?
O15 La K2 O16 12.7(5) . . . . ?
O19 La K2 O16 -95.6(5) . . . . ?
O6 La K2 O16 151.5(3) 15 . . . ?
O23 La K2 O16 -84.2(4) . . . . ?
O8 La K2 O16 58.4(4) . . . . ?
N1 La K2 O16 -14.2(4) . . . . ?
N3 La K2 O16 31.9(10) . . . . ?
K1 La K2 O16 87.2(4) 15 . . . ?
O17 La K2 C4 130.1(5) 15 . . . ?
O16 La K2 C4 -152.9(4) 15 . . . ?
O15 La K2 C4 16.0(6) . . . . ?
O19 La K2 C4 -92.4(5) . . . . ?
O6 La K2 C4 154.7(4) 15 . . . ?
O23 La K2 C4 -81.0(4) . . . . ?
O8 La K2 C4 61.6(4) . . . . ?
N1 La K2 C4 -11.0(4) . . . . ?
N3 La K2 C4 35.2(10) . . . . ?
K1 La K2 C4 90.4(4) 15 . . . ?
O17 La K2 O25 -133(2) 15 . . 3_565 ?
O16 La K2 O25 -56(2) 15 . . 3_565 ?
O15 La K2 O25 112(2) . . . 3_565 ?
O19 La K2 O25 4(2) . . . 3_565 ?
O6 La K2 O25 -109(2) 15 . . 3_565 ?
O23 La K2 O25 15(2) . . . 3_565 ?
O8 La K2 O25 158(2) . . . 3_565 ?
N1 La K2 O25 85(2) . . . 3_565 ?
N3 La K2 O25 132(2) . . . 3_565 ?
K1 La K2 O25 -173(2) 15 . . 3_565 ?
O17 La K2 K1 39.7(2) 15 . . 15 ?
O16 La K2 K1 116.7(3) 15 . . 15 ?
O15 La K2 K1 -74.5(6) . . . 15 ?
O19 La K2 K1 177.2(3) . . . 15 ?
O6 La K2 K1 64.3(3) 15 . . 15 ?
O23 La K2 K1 -171.4(3) . . . 15 ?
O8 La K2 K1 -28.8(2) . . . 15 ?
N1 La K2 K1 -101.4(3) . . . 15 ?
N3 La K2 K1 -55.2(9) . . . 15 ?
O22 K1 O24 K2 161.7(6) 2_655 . . 14_455 ?
O20 K1 O24 K2 67.4(8) 18_545 . . 14_455 ?
O9 K1 O24 K2 -121.4(8) 14_455 . . 14_455 ?
O17 K1 O24 K2 0.3(11) . . . 14_455 ?
O18 K1 O24 K2 43.0(15) . . . 14_455 ?
O24 K1 O24 K2 151(2) 16 . . 14_455 ?
O19 K1 O24 K2 108.3(9) 18_545 . . 14_455 ?
C5 K1 O24 K2 22.2(13) . . . 14_455 ?
C9 K1 O24 K2 86.0(9) 18_545 . . 14_455 ?
O8 K1 O24 K2 -65.1(10) 14_455 . . 14_455 ?
W4 K1 O24 K2 -92.6(9) 14_455 . . 14_455 ?
O22 K1 O24 K1 11(2) 2_655 . . 16 ?
O20 K1 O24 K1 -83.3(13) 18_545 . . 16 ?
O9 K1 O24 K1 87.9(13) 14_455 . . 16 ?
O17 K1 O24 K1 -150.4(11) . . . 16 ?
O18 K1 O24 K1 -107.6(13) . . . 16 ?
O24 K1 O24 K1 0.000(2) 16 . . 16 ?
O19 K1 O24 K1 -42.4(12) 18_545 . . 16 ?
C5 K1 O24 K1 -128.5(11) . . . 16 ?
C9 K1 O24 K1 -64.7(13) 18_545 . . 16 ?
O8 K1 O24 K1 144.3(11) 14_455 . . 16 ?
W4 K1 O24 K1 116.7(12) 14_455 . . 16 ?
O17 La N1 C1 141.3(11) 15 . . . ?
O16 La N1 C1 -108.1(12) 15 . . . ?
O15 La N1 C1 175.8(13) . . . . ?
O19 La N1 C1 -36.3(12) . . . . ?
O6 La N1 C1 28.1(14) 15 . . . ?
O23 La N1 C1 -105.1(12) . . . . ?
O8 La N1 C1 95.3(12) . . . . ?
N3 La N1 C1 25.5(11) . . . . ?
K1 La N1 C1 134.9(11) 15 . . . ?
K2 La N1 C1 -169.9(12) . . . . ?
O17 La N1 C2 -44.5(9) 15 . . . ?
O16 La N1 C2 66.1(9) 15 . . . ?
O15 La N1 C2 -10.1(7) . . . . ?
O19 La N1 C2 137.9(8) . . . . ?
O6 La N1 C2 -157.8(7) 15 . . . ?
O23 La N1 C2 69.0(8) . . . . ?
O8 La N1 C2 -90.5(8) . . . . ?
N3 La N1 C2 -160.4(8) . . . . ?
K1 La N1 C2 -50.9(7) 15 . . . ?
K2 La N1 C2 4.3(8) . . . . ?
O17 La N3 C6 -34.2(13) 15 . . . ?
O16 La N3 C6 -120.5(12) 15 . . . ?
O15 La N3 C6 61.9(13) . . . . ?
O19 La N3 C6 -171.5(13) . . . . ?
O6 La N3 C6 -80.9(12) 15 . . . ?
O23 La N3 C6 155.2(12) . . . . ?
O8 La N3 C6 20.9(12) . . . . ?
N1 La N3 C6 97.3(12) . . . . ?
K1 La N3 C6 3.0(13) 15 . . . ?
K2 La N3 C6 49.7(17) . . . . ?
O17 La N3 C8 123.4(8) 15 . . . ?
O16 La N3 C8 37.0(9) 15 . . . ?
O15 La N3 C8 -140.6(7) . . . . ?
O19 La N3 C8 -13.9(7) . . . . ?
O6 La N3 C8 76.7(8) 15 . . . ?
O23 La N3 C8 -47.3(9) . . . . ?
O8 La N3 C8 178.5(9) . . . . ?
N1 La N3 C8 -105.1(8) . . . . ?
K1 La N3 C8 160.6(7) 15 . . . ?
K2 La N3 C8 -152.7(8) . . . . ?
C2 N1 C1 N2 -0.6(13) . . . . ?
La N1 C1 N2 173.9(8) . . . . ?
C3 N2 C1 N1 -0.7(14) . . . . ?
C1 N1 C2 C3 1.7(13) . . . . ?
La N1 C2 C3 -174.2(7) . . . . ?
C1 N1 C2 C4 -172.0(10) . . . . ?
La N1 C2 C4 12.1(12) . . . . ?
C1 N2 C3 C2 1.7(13) . . . . ?
C1 N2 C3 C5 -178.0(10) . . . . ?
N1 C2 C3 N2 -2.0(13) . . . . ?
C4 C2 C3 N2 170.2(12) . . . . ?
N1 C2 C3 C5 177.5(12) . . . . ?
C4 C2 C3 C5 -10(2) . . . . ?
La O16 C4 O15 163.3(13) 14_455 . . . ?
K2 O16 C4 O15 -25.4(11) . . . . ?
La O16 C4 C2 -14(3) 14_455 . . . ?
K2 O16 C4 C2 157.0(11) . . . . ?
La O16 C4 K2 -171.4(19) 14_455 . . . ?
La O15 C4 O16 176.6(8) . . . . ?
K2 O15 C4 O16 28.5(13) . . . . ?
La O15 C4 C2 -5.6(15) . . . . ?
K2 O15 C4 C2 -153.8(9) . . . . ?
La O15 C4 K2 148.1(10) . . . . ?
C3 C2 C4 O16 1(2) . . . . ?
N1 C2 C4 O16 172.4(10) . . . . ?
C3 C2 C4 O15 -177.0(12) . . . . ?
N1 C2 C4 O15 -5.3(16) . . . . ?
C3 C2 C4 K2 113(2) . . . . ?
N1 C2 C4 K2 -75(2) . . . . ?
O15 K2 C4 O16 -154.1(12) . . . . ?
O12 K2 C4 O16 -53.3(13) 10_665 . . . ?
O24 K2 C4 O16 -66.9(10) 15 . . . ?
O23 K2 C4 O16 6.9(7) 14_455 . . . ?
O25 K2 C4 O16 135(2) . . . . ?
O25 K2 C4 O16 44.9(16) 3_565 . . . ?
K1 K2 C4 O16 -106.1(7) 15 . . . ?
La K2 C4 O16 -172.2(9) . . . . ?
O12 K2 C4 O15 100.8(13) 10_665 . . . ?
O24 K2 C4 O15 87.1(10) 15 . . . ?
O23 K2 C4 O15 160.9(9) 14_455 . . . ?
O25 K2 C4 O15 -71(2) . . . . ?
O16 K2 C4 O15 154.1(12) . . . . ?
O25 K2 C4 O15 -161.0(17) 3_565 . . . ?
K1 K2 C4 O15 48.0(7) 15 . . . ?
La K2 C4 O15 -18.1(6) . . . . ?
O15 K2 C4 C2 84(2) . . . . ?
O12 K2 C4 C2 -175.6(18) 10_665 . . . ?
O24 K2 C4 C2 171(2) 15 . . . ?
O23 K2 C4 C2 -116(2) 14_455 . . . ?
O25 K2 C4 C2 13(4) . . . . ?
O16 K2 C4 C2 -122(2) . . . . ?
O25 K2 C4 C2 -77(3) 3_565 . . . ?
K1 K2 C4 C2 132(2) 15 . . . ?
La K2 C4 C2 65(2) . . . . ?
La O17 C5 O18 -117.1(13) 14_455 . . . ?
K1 O17 C5 O18 32.4(14) . . . . ?
La O17 C5 C3 65.8(16) 14_455 . . . ?
K1 O17 C5 C3 -144.6(9) . . . . ?
La O17 C5 K1 -149.6(13) 14_455 . . . ?
K1 O18 C5 O17 -28.8(12) . . . . ?
K1 O18 C5 C3 148.3(9) . . . . ?
N2 C3 C5 O17 171.4(11) . . . . ?
C2 C3 C5 O17 -8(2) . . . . ?
N2 C3 C5 O18 -5.9(16) . . . . ?
C2 C3 C5 O18 174.6(13) . . . . ?
N2 C3 C5 K1 93.2(18) . . . . ?
C2 C3 C5 K1 -86(2) . . . . ?
O24 K1 C5 O17 -65.7(11) . . . . ?
O22 K1 C5 O17 140.7(7) 2_655 . . . ?
O20 K1 C5 O17 -111.8(8) 18_545 . . . ?
O9 K1 C5 O17 69.1(8) 14_455 . . . ?
O18 K1 C5 O17 152.7(12) . . . . ?
O24 K1 C5 O17 -129.3(11) 16 . . . ?
O19 K1 C5 O17 -150.3(7) 18_545 . . . ?
C9 K1 C5 O17 -135.2(8) 18_545 . . . ?
O8 K1 C5 O17 44.5(7) 14_455 . . . ?
W4 K1 C5 O17 52.0(7) 14_455 . . . ?
O24 K1 C5 O18 141.6(10) . . . . ?
O22 K1 C5 O18 -12.0(7) 2_655 . . . ?
O20 K1 C5 O18 95.5(7) 18_545 . . . ?
O9 K1 C5 O18 -83.6(8) 14_455 . . . ?
O17 K1 C5 O18 -152.7(12) . . . . ?
O24 K1 C5 O18 78.0(11) 16 . . . ?
O19 K1 C5 O18 57.0(7) 18_545 . . . ?
C9 K1 C5 O18 72.1(7) 18_545 . . . ?
O8 K1 C5 O18 -108.2(7) 14_455 . . . ?
W4 K1 C5 O18 -100.7(7) 14_455 . . . ?
O24 K1 C5 C3 31(2) . . . . ?
O22 K1 C5 C3 -122.9(17) 2_655 . . . ?
O20 K1 C5 C3 -15.4(16) 18_545 . . . ?
O9 K1 C5 C3 165.4(16) 14_455 . . . ?
O17 K1 C5 C3 96.4(19) . . . . ?
O18 K1 C5 C3 -111(2) . . . . ?
O24 K1 C5 C3 -33(2) 16 . . . ?
O19 K1 C5 C3 -53.9(17) 18_545 . . . ?
C9 K1 C5 C3 -38.9(17) 18_545 . . . ?
O8 K1 C5 C3 140.8(18) 14_455 . . . ?
W4 K1 C5 C3 148.4(17) 14_455 . . . ?
C8 N3 C6 N4 -0.3(14) . . . . ?
La N3 C6 N4 158.5(9) . . . . ?
C7 N4 C6 N3 0.0(15) . . . . ?
C6 N4 C7 C8 0.4(14) . . . . ?
C6 N4 C7 C10 -177.3(11) . . . . ?
N4 C7 C8 N3 -0.6(14) . . . . ?
C10 C7 C8 N3 176.7(13) . . . . ?
N4 C7 C8 C9 178.9(12) . . . . ?
C10 C7 C8 C9 -4(2) . . . . ?
C6 N3 C8 C7 0.5(14) . . . . ?
La N3 C8 C7 -164.9(8) . . . . ?
C6 N3 C8 C9 -179.0(10) . . . . ?
La N3 C8 C9 15.6(13) . . . . ?
La O19 C9 O20 171.6(9) . . . . ?
K1 O19 C9 O20 -31.7(12) 17 . . . ?
La O19 C9 C8 -10.6(15) . . . . ?
K1 O19 C9 C8 146.0(10) 17 . . . ?
La O19 C9 K1 -156.6(7) . . . 17 ?
K1 O20 C9 O19 38.4(14) 17 . . . ?
K1 O20 C9 C8 -139.4(9) 17 . . . ?
C7 C8 C9 O19 175.2(13) . . . . ?
N3 C8 C9 O19 -5.4(17) . . . . ?
C7 C8 C9 O20 -7(2) . . . . ?
N3 C8 C9 O20 172.5(11) . . . . ?
C7 C8 C9 K1 -75.3(19) . . . 17 ?
N3 C8 C9 K1 104.2(16) . . . 17 ?
K1 O22 C10 O21 -137.8(11) 3_665 . . . ?
K1 O22 C10 C7 45(2) 3_665 . . . ?
C8 C7 C10 O22 -176.6(13) . . . . ?
N4 C7 C10 O22 0(2) . . . . ?
C8 C7 C10 O21 6(2) . . . . ?
N4 C7 C10 O21 -176.7(11) . . . . ?
O15 K2 O25 K2 -46(7) . . . 2_665 ?
O12 K2 O25 K2 171(6) 10_665 . . 2_665 ?
O24 K2 O25 K2 -166(5) 15 . . 2_665 ?
O23 K2 O25 K2 104(6) 14_455 . . 2_665 ?
O16 K2 O25 K2 33(8) . . . 2_665 ?
C4 K2 O25 K2 -15(7) . . . 2_665 ?
O25 K2 O25 K2 99(6) 3_565 . . 2_665 ?
K1 K2 O25 K2 -119(5) 15 . . 2_665 ?
La K2 O25 K2 -53(6) . . . 2_665 ?

_diffrn_measured_fraction_theta_max 0.989
_diffrn_reflns_theta_full        23.45
_diffrn_measured_fraction_theta_full 0.989
_refine_diff_density_max         1.928
_refine_diff_density_min         -1.278
_refine_diff_density_rms         0.248
_database_code_depnum_ccdc_archive 'CCDC 828025'
#######################################################################
#
#                 Cambridge Crystallographic Data Centre
#                                CCDC 
# 
#######################################################################
# 
#  This CIF contains data from an original supplementary publication
#  deposited with the CCDC, and may include chemical, crystal,
#  experimental, refinement, atomic coordinates,
#  anisotropic displacement parameters and molecular geometry data,
#  as required by the journal to which it was submitted.
#
#  This CIF is provided on the understanding that it is used for bona
#  fide research purposes only. It may contain copyright material
#  of the CCDC or of third parties, and may not be copied or further
#  disseminated in any form, whether machine-readable or not,
#  except for the purpose of generating routine backup copies
#  on your local computer system.
# 
#  For further information on the CCDC, data deposition and
#  data retrieval see:
#                         www.ccdc.cam.ac.uk
#
#  Bona fide researchers may freely download Mercury and enCIFer
#  from this site to visualise CIF-encoded structures and 
#  to carry out CIF format checking respectively.
#
data_2

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
;
 ?
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         C30H33K4Ce3N12O73SiW12
_chemical_formula_sum            'C30 H33 K4 Ce3 N12 O73 Si W12'
_chemical_formula_weight         4540.53

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ce Ce -0.2486 2.6331 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           rhombohedral
_symmetry_space_group_name_H-M   R-3
_symmetry_space_group_name_Hall  '-R 3'

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'x+2/3, y+1/3, z+1/3'
'-y+2/3, x-y+1/3, z+1/3'
'-x+y+2/3, -x+1/3, z+1/3'
'x+1/3, y+2/3, z+2/3'
'-y+1/3, x-y+2/3, z+2/3'
'-x+y+1/3, -x+2/3, z+2/3'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'-x+2/3, -y+1/3, -z+1/3'
'y+2/3, -x+y+1/3, -z+1/3'
'x-y+2/3, x+1/3, -z+1/3'
'-x+1/3, -y+2/3, -z+2/3'
'y+1/3, -x+y+2/3, -z+2/3'
'x-y+1/3, x+2/3, -z+2/3'

_cell_length_a                   22.1520(4)
_cell_length_b                   22.1520(4)
_cell_length_c                   28.2012(12)
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_volume                     11984.6(6)
_cell_formula_units_Z            6
_cell_measurement_temperature    296(2)
_cell_measurement_reflns_used    .
_cell_measurement_theta_min      .
_cell_measurement_theta_max      .

_exptl_crystal_description       block
_exptl_crystal_colour            yellow
_exptl_crystal_size_max          0.10
_exptl_crystal_size_mid          0.08
_exptl_crystal_size_min          0.08
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    3.774
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             11968
_exptl_absorpt_coefficient_mu    19.219
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.180
_exptl_absorpt_correction_T_max  0.218
_exptl_absorpt_process_details   'SADABS (Sheldrick, 2001)'

_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_detector_area_resol_mean .
_diffrn_standards_number         .
_diffrn_standards_interval_count .
_diffrn_standards_interval_time  .
_diffrn_standards_decay_%        .
_diffrn_reflns_number            90136
_diffrn_reflns_av_R_equivalents  0.0658
_diffrn_reflns_av_sigmaI/netI    0.0207
_diffrn_reflns_limit_h_min       -27
_diffrn_reflns_limit_h_max       27
_diffrn_reflns_limit_k_min       -27
_diffrn_reflns_limit_k_max       27
_diffrn_reflns_limit_l_min       -34
_diffrn_reflns_limit_l_max       34
_diffrn_reflns_theta_min         2.17
_diffrn_reflns_theta_max         26.00
_reflns_number_total             5214
_reflns_number_gt                4769
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       'SMART (Bruker, 2007)'
_computing_cell_refinement       'SMART (Bruker, 2007)'
_computing_data_reduction        'SMART (Bruker, 2007)'
_computing_structure_solution    'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    'SHELXL-97 (Sheldrick, 1997)'
_computing_publication_material  'SHELXL-97 (Sheldrick, 1997)'

_refine_special_details          
;
 Refinement of F² against ALL reflections.  The weighted R-factor wR and
 goodness of fit S are based on F², conventional R-factors R are based
 on F, with F set to zero for negative F². The threshold expression of
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is
 not relevant to the choice of reflections for refinement.  R-factors based
 on F² are statistically about twice as large as those based on F, and R-
 factors based on ALL data will be even larger.
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0189P)²+440.2102P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_number_reflns         5214
_refine_ls_number_parameters     401
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0269
_refine_ls_R_factor_gt           0.0227
_refine_ls_wR_factor_ref         0.0533
_refine_ls_wR_factor_gt          0.0513
_refine_ls_goodness_of_fit_ref   1.012
_refine_ls_restrained_S_all      1.012
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Si Si 0.6667 0.3333 0.15046(11) 0.0163(6) Uani 1 3 d S . .
W1 W 0.714373(13) 0.434301(12) 0.255217(8) 0.01223(6) Uani 1 1 d . . .
W2 W 0.511856(12) 0.339814(12) 0.149015(8) 0.01128(6) Uani 1 1 d . . .
W3 W 0.608834(13) 0.386433(13) 0.049846(9) 0.01468(7) Uani 1 1 d . . .
W4 W 0.663034(13) 0.490219(12) 0.146193(9) 0.01230(6) Uani 1 1 d . . .
Ce Ce 0.642807(18) 0.660812(18) 0.192614(13) 0.01481(8) Uani 1 1 d . . .
K1 K 0.24565(11) 0.29378(11) 0.28600(8) 0.0532(6) Uani 1 1 d . . .
O1 O 0.6266(2) 0.3738(2) 0.13090(15) 0.0143(9) Uani 1 1 d . . .
O2 O 0.6667 0.3333 0.2082(3) 0.0120(15) Uani 1 3 d S . .
O3 O 0.7473(2) 0.3753(2) 0.28111(15) 0.0161(9) Uani 1 1 d . . .
O4 O 0.7454(3) 0.4999(2) 0.29561(16) 0.0219(10) Uani 1 1 d . . .
O5 O 0.6743(2) 0.4672(2) 0.20932(15) 0.0153(9) Uani 1 1 d . . .
O6 O 0.4291(2) 0.3268(2) 0.15606(17) 0.0198(10) Uani 1 1 d . . .
O7 O 0.5635(2) 0.4376(2) 0.15739(16) 0.0174(9) Uani 1 1 d . . .
O8 O 0.6751(2) 0.5730(2) 0.15174(16) 0.0174(9) Uani 1 1 d . . .
O9 O 0.6424(2) 0.4770(2) 0.07999(16) 0.0179(9) Uani 1 1 d . . .
O10 O 0.5220(2) 0.3563(2) 0.08148(16) 0.0175(9) Uani 1 1 d . . .
O11 O 0.4927(2) 0.2468(2) 0.13524(15) 0.0158(9) Uani 1 1 d . . .
O12 O 0.5908(3) 0.4056(3) -0.00476(16) 0.0249(11) Uani 1 1 d . . .
O13 O 0.5890(2) 0.2935(2) 0.04352(16) 0.0189(10) Uani 1 1 d . . .
O14 O 0.5322(2) 0.3234(2) 0.21056(15) 0.0148(9) Uani 1 1 d . . .
O15 O 0.5328(2) 0.5675(2) 0.15600(18) 0.0246(11) Uani 1 1 d . . .
O16 O 0.4332(3) 0.4666(2) 0.15366(18) 0.0272(12) Uani 1 1 d . . .
O17 O 0.3574(2) 0.3648(3) 0.22557(17) 0.0252(11) Uani 1 1 d . . .
O18 O 0.3976(3) 0.3283(3) 0.28429(19) 0.0298(12) Uani 1 1 d . . .
O19 O 0.6782(3) 0.7141(3) 0.27454(18) 0.0286(12) Uani 1 1 d . . .
O20 O 0.7502(3) 0.7597(3) 0.33546(17) 0.0257(11) Uani 1 1 d . . .
O21 O 0.8673(3) 0.7807(3) 0.35862(19) 0.0329(12) Uani 1 1 d . . .
H21 H 0.8284 0.7732 0.3511 0.049 Uiso 1 1 calc R . .
O22 O 0.9401(3) 0.7465(3) 0.3361(2) 0.0350(13) Uani 1 1 d . . .
O23 O 0.5382(3) 0.6567(3) 0.23858(19) 0.0294(12) Uani 1 1 d . . .
K2 K 0.4450(5) 0.5893(5) 0.0988(3) 0.071(2) Uiso 0.33 1 d P . .
O24 O 0.1757(9) 0.3623(9) 0.2922(6) 0.076(5) Uiso 0.50 1 d P . .
N1 N 0.5731(3) 0.5390(3) 0.23862(19) 0.0163(11) Uani 1 1 d . . .
N2 N 0.5234(3) 0.4478(3) 0.28487(19) 0.0191(12) Uani 1 1 d . . .
H2 H 0.5180 0.4197 0.3077 0.023 Uiso 1 1 calc R . .
N3 N 0.7498(3) 0.6531(3) 0.2392(2) 0.0198(12) Uani 1 1 d . . .
N4 N 0.8494(3) 0.6633(3) 0.2626(2) 0.0230(13) Uani 1 1 d . . .
H4 H 0.8853 0.6579 0.2632 0.028 Uiso 1 1 calc R . .
C1 C 0.5806(3) 0.5093(3) 0.2774(2) 0.0189(13) Uani 1 1 d . . .
H1 H 0.6201 0.5287 0.2966 0.023 Uiso 1 1 calc R . .
C2 C 0.5071(3) 0.4933(3) 0.2213(2) 0.0137(12) Uani 1 1 d . . .
C3 C 0.4751(3) 0.4361(3) 0.2510(2) 0.0152(12) Uani 1 1 d . . .
C4 C 0.4882(3) 0.5089(3) 0.1744(2) 0.0167(13) Uani 1 1 d . . .
C5 C 0.4047(3) 0.3713(3) 0.2534(2) 0.0175(13) Uani 1 1 d . . .
C6 C 0.7969(4) 0.6343(4) 0.2318(3) 0.0238(15) Uani 1 1 d . . .
H6 H 0.7938 0.6041 0.2078 0.029 Uiso 1 1 calc R . .
C7 C 0.8356(4) 0.7035(4) 0.2932(2) 0.0210(14) Uani 1 1 d . . .
C8 C 0.7739(3) 0.6966(3) 0.2779(2) 0.0191(14) Uani 1 1 d . . .
C9 C 0.7318(4) 0.7266(4) 0.2970(2) 0.0213(14) Uani 1 1 d . . .
C10 C 0.8852(4) 0.7458(4) 0.3312(3) 0.0266(16) Uani 1 1 d . . .
O25B O 0.4256(16) 0.7155(16) 0.0771(11) 0.093(9) Uiso 0.33 1 d P . .
O25A O 0.4034(16) 0.5936(16) 0.2011(11) 0.088(8) Uiso 0.33 1 d P . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Si O2 1.628(8) . ?
Si O1 1.640(4) 2_655 ?
Si O1 1.640(4) 3_665 ?
Si O1 1.640(4) . ?
W1 O4 1.698(4) . ?
W1 O5 1.907(4) . ?
W1 O3 1.908(4) 2_655 ?
W1 O3 1.931(4) . ?
W1 O14 1.942(4) 3_665 ?
W1 O2 2.349(4) . ?
W2 O6 1.718(4) . ?
W2 O14 1.874(4) . ?
W2 O7 1.893(4) . ?
W2 O11 1.924(4) . ?
W2 O10 1.931(4) . ?
W2 O1 2.318(4) . ?
W3 O12 1.697(4) . ?
W3 O13 1.887(4) . ?
W3 O10 1.913(4) . ?
W3 O13 1.913(4) 3_665 ?
W3 O9 1.952(4) . ?
W3 O1 2.360(4) . ?
W4 O8 1.722(4) . ?
W4 O11 1.883(4) 3_665 ?
W4 O5 1.903(4) . ?
W4 O9 1.909(4) . ?
W4 O7 1.936(4) . ?
W4 O1 2.326(4) . ?
W4 K1 3.814(2) 15 ?
Ce O17 2.461(5) 15 ?
Ce O16 2.482(5) 15 ?
Ce O15 2.499(4) . ?
Ce O19 2.534(5) . ?
Ce O6 2.604(4) 15 ?
Ce O23 2.616(5) . ?
Ce O8 2.650(4) . ?
Ce N1 2.679(5) . ?
Ce N3 2.790(6) . ?
Ce K1 4.403(2) 15 ?
K1 O24 2.663(18) . ?
K1 O22 2.707(6) 2_655 ?
K1 O20 2.709(5) 18_545 ?
K1 O9 2.725(5) 14_455 ?
K1 O17 2.759(5) . ?
K1 O18 3.058(6) . ?
K1 C5 3.187(7) . ?
K1 O19 3.202(6) 18_545 ?
K1 C9 3.226(7) 18_545 ?
K1 O8 3.229(5) 14_455 ?
K1 O24 3.246(18) 16 ?
K1 W4 3.814(2) 14_455 ?
O2 W1 2.349(4) 3_665 ?
O2 W1 2.349(4) 2_655 ?
O3 W1 1.908(4) 3_665 ?
O6 Ce 2.604(4) 14_455 ?
O8 K1 3.229(5) 15 ?
O9 K1 2.725(5) 15 ?
O11 W4 1.883(4) 2_655 ?
O12 K2 2.786(10) 10_665 ?
O13 W3 1.913(4) 2_655 ?
O14 W1 1.942(4) 2_655 ?
O15 C4 1.282(8) . ?
O15 K2 2.749(10) . ?
O16 C4 1.249(8) . ?
O16 Ce 2.482(5) 14_455 ?
O16 K2 3.022(10) . ?
O17 C5 1.259(8) . ?
O17 Ce 2.461(5) 14_455 ?
O18 C5 1.241(8) . ?
O19 C9 1.250(8) . ?
O19 K1 3.202(6) 17 ?
O20 C9 1.257(8) . ?
O20 K1 2.709(5) 17 ?
O21 C10 1.288(9) . ?
O22 C10 1.216(9) . ?
O22 K1 2.707(6) 3_665 ?
O23 K2 2.887(10) 15 ?
K2 O12 2.786(10) 10_665 ?
K2 O24 2.79(2) 15 ?
K2 O23 2.887(10) 14_455 ?
K2 O25A 3.04(3) . ?
K2 O25B 3.10(3) . ?
K2 O25A 3.13(3) 15 ?
K2 C4 3.215(11) . ?
K2 O25B 3.34(3) 3_565 ?
K2 K1 4.221(9) 15 ?
O24 K2 2.79(2) 14_455 ?
O24 K1 3.246(18) 16 ?
N1 C1 1.329(8) . ?
N1 C2 1.386(8) . ?
N2 C1 1.335(9) . ?
N2 C3 1.360(8) . ?
N3 C6 1.319(9) . ?
N3 C8 1.374(9) . ?
N4 C6 1.330(9) . ?
N4 C7 1.381(9) . ?
C2 C3 1.382(9) . ?
C2 C4 1.482(9) . ?
C3 C5 1.503(9) . ?
C7 C8 1.368(9) . ?
C7 C10 1.486(10) . ?
C8 C9 1.490(10) . ?
C9 K1 3.226(7) 17 ?
O25B K2 3.34(3) 2_665 ?
O25A K2 3.13(3) 14_455 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O2 Si O1 109.66(18) . 2_655 ?
O2 Si O1 109.66(18) . 3_665 ?
O1 Si O1 109.29(18) 2_655 3_665 ?
O2 Si O1 109.66(18) . . ?
O1 Si O1 109.29(18) 2_655 . ?
O1 Si O1 109.29(18) 3_665 . ?
O4 W1 O5 101.3(2) . . ?
O4 W1 O3 101.0(2) . 2_655 ?
O5 W1 O3 91.19(19) . 2_655 ?
O4 W1 O3 101.4(2) . . ?
O5 W1 O3 156.97(18) . . ?
O3 W1 O3 88.6(3) 2_655 . ?
O4 W1 O14 101.9(2) . 3_665 ?
O5 W1 O14 84.27(18) . 3_665 ?
O3 W1 O14 157.08(18) 2_655 3_665 ?
O3 W1 O14 87.00(18) . 3_665 ?
O4 W1 O2 172.3(2) . . ?
O5 W1 O2 84.63(17) . . ?
O3 W1 O2 73.61(16) 2_655 . ?
O3 W1 O2 73.23(16) . . ?
O14 W1 O2 83.58(17) 3_665 . ?
O6 W2 O14 101.6(2) . . ?
O6 W2 O7 99.3(2) . . ?
O14 W2 O7 92.28(19) . . ?
O6 W2 O11 101.4(2) . . ?
O14 W2 O11 85.70(18) . . ?
O7 W2 O11 159.19(19) . . ?
O6 W2 O10 99.2(2) . . ?
O14 W2 O10 158.99(19) . . ?
O7 W2 O10 87.73(19) . . ?
O11 W2 O10 86.89(18) . . ?
O6 W2 O1 169.80(19) . . ?
O14 W2 O1 86.30(17) . . ?
O7 W2 O1 73.66(17) . . ?
O11 W2 O1 85.53(17) . . ?
O10 W2 O1 73.53(17) . . ?
O12 W3 O13 103.4(2) . . ?
O12 W3 O10 100.9(2) . . ?
O13 W3 O10 91.06(19) . . ?
O12 W3 O13 102.1(2) . 3_665 ?
O13 W3 O13 85.5(3) . 3_665 ?
O10 W3 O13 156.90(19) . 3_665 ?
O12 W3 O9 98.9(2) . . ?
O13 W3 O9 157.52(19) . . ?
O10 W3 O9 87.48(19) . . ?
O13 W3 O9 87.12(19) 3_665 . ?
O12 W3 O1 169.3(2) . . ?
O13 W3 O1 85.60(17) . . ?
O10 W3 O1 72.85(17) . . ?
O13 W3 O1 84.11(17) 3_665 . ?
O9 W3 O1 72.54(16) . . ?
O8 W4 O11 102.7(2) . 3_665 ?
O8 W4 O5 103.3(2) . . ?
O11 W4 O5 86.33(18) 3_665 . ?
O8 W4 O9 98.6(2) . . ?
O11 W4 O9 91.17(19) 3_665 . ?
O5 W4 O9 157.98(18) . . ?
O8 W4 O7 98.6(2) . . ?
O11 W4 O7 158.59(18) 3_665 . ?
O5 W4 O7 87.07(19) . . ?
O9 W4 O7 87.38(19) . . ?
O8 W4 O1 168.66(18) . . ?
O11 W4 O1 86.30(17) 3_665 . ?
O5 W4 O1 83.97(17) . . ?
O9 W4 O1 74.04(17) . . ?
O7 W4 O1 72.76(17) . . ?
O8 W4 K1 57.34(15) . 15 ?
O11 W4 K1 107.67(13) 3_665 15 ?
O5 W4 K1 157.64(13) . 15 ?
O9 W4 K1 42.34(13) . 15 ?
O7 W4 K1 85.38(14) . 15 ?
O1 W4 K1 113.61(11) . 15 ?
O17 Ce O16 70.98(16) 15 15 ?
O17 Ce O15 76.90(16) 15 . ?
O16 Ce O15 102.24(17) 15 . ?
O17 Ce O19 142.32(17) 15 . ?
O16 Ce O19 81.21(17) 15 . ?
O15 Ce O19 135.13(17) . . ?
O17 Ce O6 69.81(16) 15 15 ?
O16 Ce O6 73.79(16) 15 15 ?
O15 Ce O6 145.95(16) . 15 ?
O19 Ce O6 78.49(16) . 15 ?
O17 Ce O23 120.06(17) 15 . ?
O16 Ce O23 67.28(16) 15 . ?
O15 Ce O23 72.28(17) . . ?
O19 Ce O23 68.07(17) . . ?
O6 Ce O23 131.42(16) 15 . ?
O17 Ce O8 73.53(15) 15 . ?
O16 Ce O8 144.19(15) 15 . ?
O15 Ce O8 73.89(16) . . ?
O19 Ce O8 127.19(15) . . ?
O6 Ce O8 89.73(14) 15 . ?
O23 Ce O8 138.57(15) . . ?
O17 Ce N1 132.48(16) 15 . ?
O16 Ce N1 137.99(16) 15 . ?
O15 Ce N1 62.24(16) . . ?
O19 Ce N1 85.15(17) . . ?
O6 Ce N1 141.29(15) 15 . ?
O23 Ce N1 70.76(16) . . ?
O8 Ce N1 72.70(15) . . ?
O17 Ce N3 117.27(17) 15 . ?
O16 Ce N3 127.12(18) 15 . ?
O15 Ce N3 130.62(16) . . ?
O19 Ce N3 61.62(16) . . ?
O6 Ce N3 63.48(15) 15 . ?
O23 Ce N3 121.95(17) . . ?
O8 Ce N3 67.04(15) . . ?
N1 Ce N3 77.85(16) . . ?
O17 Ce K1 34.64(11) 15 15 ?
O16 Ce K1 101.61(12) 15 15 ?
O15 Ce K1 53.63(13) . 15 ?
O19 Ce K1 170.37(12) . 15 ?
O6 Ce K1 93.37(11) 15 15 ?
O23 Ce K1 121.54(13) . 15 ?
O8 Ce K1 46.77(10) . 15 ?
N1 Ce K1 98.39(12) . 15 ?
N3 Ce K1 110.22(12) . 15 ?
O24 K1 O22 136.7(4) . 2_655 ?
O24 K1 O20 70.0(4) . 18_545 ?
O22 K1 O20 107.96(18) 2_655 18_545 ?
O24 K1 O9 100.6(4) . 14_455 ?
O22 K1 O9 72.42(16) 2_655 14_455 ?
O20 K1 O9 167.09(17) 18_545 14_455 ?
O24 K1 O17 109.1(4) . . ?
O22 K1 O17 112.45(18) 2_655 . ?
O20 K1 O17 77.11(16) 18_545 . ?
O9 K1 O17 115.02(16) 14_455 . ?
O24 K1 O18 137.8(4) . . ?
O22 K1 O18 72.48(16) 2_655 . ?
O20 K1 O18 71.67(16) 18_545 . ?
O9 K1 O18 119.75(16) 14_455 . ?
O17 K1 O18 44.42(14) . . ?
O24 K1 C5 120.9(4) . . ?
O22 K1 C5 94.87(18) 2_655 . ?
O20 K1 C5 67.35(16) 18_545 . ?
O9 K1 C5 125.54(17) 14_455 . ?
O17 K1 C5 23.03(16) . . ?
O18 K1 C5 22.81(15) . . ?
O24 K1 O19 86.9(4) . 18_545 ?
O22 K1 O19 69.12(16) 2_655 18_545 ?
O20 K1 O19 43.01(14) 18_545 18_545 ?
O9 K1 O19 130.12(15) 14_455 18_545 ?
O17 K1 O19 108.37(15) . 18_545 ?
O18 K1 O19 76.78(15) . 18_545 ?
C5 K1 O19 88.56(16) . 18_545 ?
O24 K1 C9 83.5(4) . 18_545 ?
O22 K1 C9 85.89(18) 2_655 18_545 ?
O20 K1 C9 22.35(16) 18_545 18_545 ?
O9 K1 C9 152.52(18) 14_455 18_545 ?
O17 K1 C9 88.50(17) . 18_545 ?
O18 K1 C9 66.73(16) . 18_545 ?
C5 K1 C9 71.79(17) . 18_545 ?
O19 K1 C9 22.41(15) 18_545 18_545 ?
O24 K1 O8 113.2(4) . 14_455 ?
O22 K1 O8 97.43(15) 2_655 14_455 ?
O20 K1 O8 136.86(15) 18_545 14_455 ?
O9 K1 O8 54.36(13) 14_455 14_455 ?
O17 K1 O8 60.93(13) . 14_455 ?
O18 K1 O8 84.07(14) . 14_455 ?
C5 K1 O8 76.44(15) . 14_455 ?
O19 K1 O8 159.15(15) 18_545 14_455 ?
C9 K1 O8 148.22(16) 18_545 14_455 ?
O24 K1 O24 50.7(6) . 16 ?
O22 K1 O24 86.8(3) 2_655 16 ?
O20 K1 O24 70.8(3) 18_545 16 ?
O9 K1 O24 96.5(3) 14_455 16 ?
O17 K1 O24 146.5(3) . 16 ?
O18 K1 O24 128.3(3) . 16 ?
C5 K1 O24 136.4(3) . 16 ?
O19 K1 O24 51.5(3) 18_545 16 ?
C9 K1 O24 64.9(3) 18_545 16 ?
O8 K1 O24 146.6(3) 14_455 16 ?
O24 K1 W4 105.5(4) . 14_455 ?
O22 K1 W4 88.08(13) 2_655 14_455 ?
O20 K1 W4 161.04(14) 18_545 14_455 ?
O9 K1 W4 28.16(10) 14_455 14_455 ?
O17 K1 W4 87.59(12) . 14_455 ?
O18 K1 W4 105.01(12) . 14_455 ?
C5 K1 W4 102.09(13) . 14_455 ?
O19 K1 W4 155.71(12) 18_545 14_455 ?
C9 K1 W4 170.98(15) 18_545 14_455 ?
O8 K1 W4 26.68(8) 14_455 14_455 ?
O24 K1 W4 121.5(3) 16 14_455 ?
Si O1 W2 123.6(2) . . ?
Si O1 W4 124.1(2) . . ?
W2 O1 W4 92.01(15) . . ?
Si O1 W3 124.0(2) . . ?
W2 O1 W3 91.78(15) . . ?
W4 O1 W3 91.92(15) . . ?
Si O2 W1 124.39(15) . 3_665 ?
Si O2 W1 124.39(15) . . ?
W1 O2 W1 91.2(2) 3_665 . ?
Si O2 W1 124.39(15) . 2_655 ?
W1 O2 W1 91.2(2) 3_665 2_655 ?
W1 O2 W1 91.2(2) . 2_655 ?
W1 O3 W1 121.9(2) 3_665 . ?
W4 O5 W1 152.4(2) . . ?
W2 O6 Ce 155.1(3) . 14_455 ?
W2 O7 W4 121.6(2) . . ?
W4 O8 Ce 150.0(2) . . ?
W4 O8 K1 95.98(18) . 15 ?
Ce O8 K1 96.51(13) . 15 ?
W4 O9 W3 121.5(2) . . ?
W4 O9 K1 109.51(19) . 15 ?
W3 O9 K1 124.9(2) . 15 ?
W3 O10 W2 121.8(2) . . ?
W4 O11 W2 150.0(2) 2_655 . ?
W3 O12 K2 168.9(3) . 10_665 ?
W3 O13 W3 151.9(3) . 2_655 ?
W2 O14 W1 152.3(2) . 2_655 ?
C4 O15 Ce 127.5(4) . . ?
C4 O15 K2 99.2(4) . . ?
Ce O15 K2 125.5(3) . . ?
C4 O16 Ce 154.8(4) . 14_455 ?
C4 O16 K2 87.3(4) . . ?
Ce O16 K2 117.5(2) 14_455 . ?
C5 O17 Ce 141.2(4) . 14_455 ?
C5 O17 K1 97.9(4) . . ?
Ce O17 K1 114.89(18) 14_455 . ?
C5 O18 K1 84.5(4) . . ?
C9 O19 Ce 127.2(4) . . ?
C9 O19 K1 79.9(4) . 17 ?
Ce O19 K1 145.8(2) . 17 ?
C9 O20 K1 102.6(4) . 17 ?
C10 O22 K1 142.0(5) . 3_665 ?
Ce O23 K2 117.8(2) . 15 ?
O15 K2 O12 143.8(4) . 10_665 ?
O15 K2 O24 77.5(4) . 15 ?
O12 K2 O24 69.4(4) 10_665 15 ?
O15 K2 O23 101.9(3) . 14_455 ?
O12 K2 O23 82.6(3) 10_665 14_455 ?
O24 K2 O23 73.5(4) 15 14_455 ?
O15 K2 O16 44.94(19) . . ?
O12 K2 O16 128.8(3) 10_665 . ?
O24 K2 O16 69.6(4) 15 . ?
O23 K2 O16 57.1(2) 14_455 . ?
O15 K2 O25A 72.6(6) . . ?
O12 K2 O25A 143.5(7) 10_665 . ?
O24 K2 O25A 139.2(7) 15 . ?
O23 K2 O25A 86.2(6) 14_455 . ?
O16 K2 O25A 69.6(6) . . ?
O15 K2 O25B 134.8(7) . . ?
O12 K2 O25B 66.7(6) 10_665 . ?
O24 K2 O25B 132.0(8) 15 . ?
O23 K2 O25B 117.9(7) 14_455 . ?
O16 K2 O25B 157.6(7) . . ?
O25A K2 O25B 88.8(8) . . ?
O15 K2 O25A 101.4(6) . 15 ?
O12 K2 O25A 99.4(6) 10_665 15 ?
O24 K2 O25A 148.6(7) 15 15 ?
O23 K2 O25A 135.8(6) 14_455 15 ?
O16 K2 O25A 131.2(6) . 15 ?
O25A K2 O25A 66.0(9) . 15 ?
O25B K2 O25A 34.4(8) . 15 ?
O15 K2 C4 23.18(16) . . ?
O12 K2 C4 145.4(4) 10_665 . ?
O24 K2 C4 77.2(4) 15 . ?
O23 K2 C4 79.7(3) 14_455 . ?
O16 K2 C4 22.84(15) . . ?
O25A K2 C4 64.4(6) . . ?
O25B K2 C4 147.8(7) . . ?
O25A K2 C4 113.9(6) 15 . ?
O15 K2 O25B 150.9(6) . 3_565 ?
O12 K2 O25B 62.0(6) 10_665 3_565 ?
O24 K2 O25B 115.5(7) 15 3_565 ?
O23 K2 O25B 61.2(6) 14_455 3_565 ?
O16 K2 O25B 112.5(6) . 3_565 ?
O25A K2 O25B 82.2(8) . 3_565 ?
O25B K2 O25B 56.8(11) . 3_565 ?
O25A K2 O25B 80.8(8) 15 3_565 ?
C4 K2 O25B 130.1(6) . 3_565 ?
O15 K2 K1 56.55(19) . 15 ?
O12 K2 K1 87.7(2) 10_665 15 ?
O24 K2 K1 38.2(4) 15 15 ?
O23 K2 K1 108.9(3) 14_455 15 ?
O16 K2 K1 78.4(2) . 15 ?
O25A K2 K1 128.7(6) . 15 ?
O25B K2 K1 121.5(6) . 15 ?
O25A K2 K1 115.3(6) 15 15 ?
C4 K2 K1 70.5(2) . 15 ?
O25B K2 K1 148.4(6) 3_565 15 ?
K1 O24 K2 101.4(6) . 14_455 ?
K1 O24 K1 129.3(6) . 16 ?
K2 O24 K1 120.8(6) 14_455 16 ?
C1 N1 C2 106.0(5) . . ?
C1 N1 Ce 138.2(4) . . ?
C2 N1 Ce 115.6(4) . . ?
C1 N2 C3 109.8(6) . . ?
C6 N3 C8 104.9(6) . . ?
C6 N3 Ce 140.9(5) . . ?
C8 N3 Ce 111.9(4) . . ?
C6 N4 C7 107.3(6) . . ?
N1 C1 N2 110.2(6) . . ?
C3 C2 N1 109.1(5) . . ?
C3 C2 C4 132.8(6) . . ?
N1 C2 C4 117.5(5) . . ?
N2 C3 C2 104.9(6) . . ?
N2 C3 C5 119.4(6) . . ?
C2 C3 C5 135.7(6) . . ?
O16 C4 O15 122.6(6) . . ?
O16 C4 C2 121.7(6) . . ?
O15 C4 C2 115.6(5) . . ?
O16 C4 K2 69.9(4) . . ?
O15 C4 K2 57.6(4) . . ?
C2 C4 K2 156.8(5) . . ?
O18 C5 O17 124.8(6) . . ?
O18 C5 C3 116.0(6) . . ?
O17 C5 C3 119.2(6) . . ?
O18 C5 K1 72.7(4) . . ?
O17 C5 K1 59.0(3) . . ?
C3 C5 K1 150.1(4) . . ?
N3 C6 N4 112.5(6) . . ?
C8 C7 N4 105.2(6) . . ?
C8 C7 C10 133.0(7) . . ?
N4 C7 C10 121.7(6) . . ?
C7 C8 N3 110.1(6) . . ?
C7 C8 C9 130.5(6) . . ?
N3 C8 C9 119.4(6) . . ?
O19 C9 O20 124.2(7) . . ?
O19 C9 C8 117.1(6) . . ?
O20 C9 C8 118.6(6) . . ?
O19 C9 K1 77.7(4) . 17 ?
O20 C9 K1 55.0(3) . 17 ?
C8 C9 K1 144.4(4) . 17 ?
O22 C10 O21 122.2(7) . . ?
O22 C10 C7 120.6(7) . . ?
O21 C10 C7 117.3(6) . . ?
K2 O25B K2 157.9(12) . 2_665 ?
K2 O25A K2 117.9(10) . 14_455 ?

_diffrn_measured_fraction_theta_max 0.993
_diffrn_reflns_theta_full        26.00
_diffrn_measured_fraction_theta_full 0.993
_refine_diff_density_max         1.951
_refine_diff_density_min         -1.455
_refine_diff_density_rms         0.189
_database_code_depnum_ccdc_archive 'CCDC 828026'
#######################################################################
#
#                 Cambridge Crystallographic Data Centre
#                                CCDC 
# 
#######################################################################
# 
#  This CIF contains data from an original supplementary publication
#  deposited with the CCDC, and may include chemical, crystal,
#  experimental, refinement, atomic coordinates,
#  anisotropic displacement parameters and molecular geometry data,
#  as required by the journal to which it was submitted.
#
#  This CIF is provided on the understanding that it is used for bona
#  fide research purposes only. It may contain copyright material
#  of the CCDC or of third parties, and may not be copied or further
#  disseminated in any form, whether machine-readable or not,
#  except for the purpose of generating routine backup copies
#  on your local computer system.
# 
#  For further information on the CCDC, data deposition and
#  data retrieval see:
#                         www.ccdc.cam.ac.uk
#
#  Bona fide researchers may freely download Mercury and enCIFer
#  from this site to visualise CIF-encoded structures and 
#  to carry out CIF format checking respectively.
#
data_la3d

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
;
 ?
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         C20H46La4N8O75SiW12
_chemical_formula_sum            'C20 H46 La4 N8 O75 Si W12'
_chemical_formula_weight         4388.38

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
La La -0.2871 2.4523 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_H-M   'p 21/c'
_symmetry_space_group_name_Hall  '-p 2ybc'

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'

_cell_length_a                   13.685(5)
_cell_length_b                   13.144(4)
_cell_length_c                   22.649(7)
_cell_angle_alpha                90.00
_cell_angle_beta                 100.551(5)
_cell_angle_gamma                90.00
_cell_volume                     4005(2)
_cell_formula_units_Z            2
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    .
_cell_measurement_theta_min      .
_cell_measurement_theta_max      .

_exptl_crystal_description       block
_exptl_crystal_colour            yellow
_exptl_crystal_size_max          0.09
_exptl_crystal_size_mid          0.06
_exptl_crystal_size_min          0.055
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    3.639
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             3796
_exptl_absorpt_coefficient_mu    19.370
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.255
_exptl_absorpt_correction_T_max  0.352
_exptl_absorpt_process_details   'SADABS (Sheldrick, 2001)'

_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_detector_area_resol_mean .
_diffrn_standards_number         .
_diffrn_standards_interval_count .
_diffrn_standards_interval_time  .
_diffrn_standards_decay_%        .
_diffrn_reflns_number            20014
_diffrn_reflns_av_R_equivalents  0.1231
_diffrn_reflns_av_sigmaI/netI    0.1640
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_l_min       -27
_diffrn_reflns_limit_l_max       27
_diffrn_reflns_theta_min         2.15
_diffrn_reflns_theta_max         25.75
_reflns_number_total             7563
_reflns_number_gt                4400
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       'SMART (Bruker, 2007)'
_computing_cell_refinement       'SMART (Bruker, 2007)'
_computing_data_reduction        'SMART (Bruker, 2007)'
_computing_structure_solution    'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    'SHELXL-97 (Sheldrick, 1997)'
_computing_publication_material  'SHELXL-97 (Sheldrick, 1997)'

_refine_special_details          
;
 Refinement of F² against ALL reflections.  The weighted R-factor wR and
 goodness of fit S are based on F², conventional R-factors R are based
 on F, with F set to zero for negative F². The threshold expression of
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is
 not relevant to the choice of reflections for refinement.  R-factors based
 on F² are statistically about twice as large as those based on F, and R-
 factors based on ALL data will be even larger.
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0948P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     SHELXL
_refine_ls_extinction_coef       0.00094(7)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_number_reflns         7563
_refine_ls_number_parameters     365
_refine_ls_number_restraints     6
_refine_ls_R_factor_all          0.1585
_refine_ls_R_factor_gt           0.0838
_refine_ls_wR_factor_ref         0.2035
_refine_ls_wR_factor_gt          0.1734
_refine_ls_goodness_of_fit_ref   1.010
_refine_ls_restrained_S_all      1.009
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Si Si 0.5000 0.5000 0.5000 0.0086(19) Uani 1 2 d SU . .
W1 W 0.23809(11) 0.48897(11) 0.47599(7) 0.0414(4) Uani 1 1 d . . .
W2 W 0.35508(10) 0.68963(9) 0.41363(6) 0.0302(4) Uani 1 1 d . . .
W3 W 0.36624(11) 0.44240(10) 0.35741(6) 0.0370(4) Uani 1 1 d . . .
W4 W 0.50929(10) 0.25307(9) 0.44144(6) 0.0318(4) Uani 1 1 d . . .
W5 W 0.38202(9) 0.30063(8) 0.56149(6) 0.0250(3) Uani 1 1 d . . .
W6 W 0.37210(10) 0.54721(10) 0.62070(6) 0.0330(4) Uani 1 1 d . . .
La1 La 0.27569(12) 0.40167(11) 0.17655(8) 0.0176(4) Uani 1 1 d . . .
La2 La 0.78086(11) 0.40149(11) 0.22202(8) 0.0199(4) Uani 1 1 d . . .
O1A O 0.403(3) 0.527(3) 0.4564(17) 0.021(8) Uiso 0.50 1 d P . .
O1B O 0.502(3) 0.615(3) 0.4841(17) 0.023(9) Uiso 0.50 1 d P . .
O2A O 0.507(3) 0.427(2) 0.4403(16) 0.016(8) Uiso 0.50 1 d P . .
O2B O 0.597(3) 0.533(3) 0.4727(18) 0.026(9) Uiso 0.50 1 d P . .
O3 O 0.132(2) 0.4813(15) 0.4693(12) 0.055(8) Uani 1 1 d . . .
O4 O 0.258(2) 0.433(2) 0.3993(12) 0.062(7) Uiso 1 1 d . . .
O5 O 0.270(2) 0.358(2) 0.5137(13) 0.068(8) Uiso 1 1 d . . .
O6 O 0.269(3) 0.539(3) 0.5563(18) 0.029(10) Uiso 0.50 1 d P . .
O7 O 0.256(2) 0.625(2) 0.4425(14) 0.083(9) Uiso 1 1 d . . .
O8 O 0.2932(16) 0.7804(17) 0.3726(10) 0.044(6) Uani 1 1 d . . .
O9 O 0.483(2) 0.7223(19) 0.3977(12) 0.060(7) Uiso 1 1 d . . .
O10 O 0.3562(18) 0.5791(18) 0.3563(11) 0.051(7) Uiso 1 1 d . . .
O11 O 0.402(3) 0.312(3) 0.3913(19) 0.033(10) Uiso 0.50 1 d P . .
O12 O 0.5164(17) 0.1342(15) 0.4146(11) 0.046(6) Uani 1 1 d . . .
O13 O 0.608(2) 0.245(3) 0.5111(13) 0.097(12) Uani 1 1 d . . .
O14 O 0.412(2) 0.236(2) 0.4921(12) 0.062(7) Uiso 1 1 d . . .
O15 O 0.333(2) 0.205(2) 0.5916(12) 0.068(8) Uani 1 1 d . . .
O16 O 0.368(2) 0.403(2) 0.6201(12) 0.063(7) Uiso 1 1 d . . .
O17 O 0.3128(18) 0.5645(16) 0.6776(10) 0.045(6) Uani 1 1 d . . .
O18 O 0.509(2) 0.539(2) 0.6593(13) 0.074(9) Uiso 1 1 d . . .
O19 O 0.397(2) 0.683(2) 0.5959(14) 0.076(9) Uiso 1 1 d . . .
O20 O 0.3033(15) 0.4129(15) 0.2897(9) 0.033(5) Uiso 1 1 d . . .
O21 O 0.127(3) 0.338(3) 0.0876(18) 0.114(13) Uiso 1 1 d . . .
O22 O 0.277(3) 0.515(3) 0.0840(16) 0.098(11) Uiso 1 1 d . . .
O23 O 0.4477(14) 0.4772(13) 0.1883(9) 0.022(4) Uiso 1 1 d . . .
O24 O 0.6088(15) 0.4527(14) 0.1929(9) 0.028(5) Uiso 1 1 d . . .
O25 O 0.7904(17) 0.7332(17) 0.2903(10) 0.042(6) Uiso 1 1 d . . .
O26 O 0.7828(14) 0.5810(14) 0.2505(9) 0.026(5) Uiso 1 1 d . . .
O27 O 0.768(2) 0.489(2) 0.1191(12) 0.063(8) Uani 1 1 d . . .
O28 O 0.9038(18) 0.4038(19) 0.3249(11) 0.055(7) Uani 1 1 d . . .
O29 O 0.7224(15) 0.2414(14) 0.2643(9) 0.030(5) Uani 1 1 d . . .
O30 O 0.7397(14) 0.0830(13) 0.2969(9) 0.026(5) Uani 1 1 d . . .
O31 O 1.0538(15) -0.0454(15) 0.2974(9) 0.030(5) Uiso 1 1 d . . .
O32 O 0.8936(14) -0.0661(14) 0.3064(9) 0.027(5) Uiso 1 1 d . . .
O33 O 0.796(8) 0.206(7) 0.445(4) 0.16(4) Uiso 0.50 1 d P . .
O34 O 1.096(3) 0.340(3) 0.3239(16) 0.097(11) Uiso 1 1 d . . .
O35 O 0.787(4) 0.689(4) 0.104(2) 0.156(18) Uiso 1 1 d . . .
O36 O 0.912(3) 0.588(3) 0.4008(18) 0.113(12) Uiso 1 1 d . . .
O37 O -0.074(6) 0.386(6) 0.068(3) 0.11(3) Uiso 0.50 1 d P . .
O38 O 0.485(2) -0.054(2) 0.4353(13) 0.069(8) Uiso 1 1 d . . .
O39 O 0.377(6) 0.000(6) 0.476(4) 0.11(3) Uiso 0.50 1 d P . .
N1 N 0.4697(17) 0.6625(16) 0.2349(10) 0.019(5) Uiso 1 1 d . . .
H1 H 0.4091 0.6435 0.2234 0.022 Uiso 1 1 calc R . .
N2 N 0.5947(17) 0.7626(17) 0.2739(10) 0.023(5) Uani 1 1 d . . .
N3 N 0.8915(17) 0.2392(17) 0.2238(10) 0.023(5) Uiso 1 1 d . . .
N4 N 1.015(2) 0.1318(19) 0.2344(12) 0.034(6) Uiso 1 1 d . . .
H4 H 1.0701 0.1043 0.2296 0.041 Uiso 1 1 calc R . .
C1 C 0.498(2) 0.748(2) 0.2600(14) 0.032(7) Uiso 1 1 d . . .
H2 H 0.4534 0.7974 0.2677 0.038 Uiso 1 1 calc R . .
C2 C 0.5523(17) 0.6071(17) 0.2298(11) 0.011(5) Uiso 1 1 d . . .
C3 C 0.6312(18) 0.6706(18) 0.2541(11) 0.012(5) Uiso 1 1 d . . .
C4 C 0.736(2) 0.662(2) 0.2660(14) 0.029(7) Uiso 1 1 d . . .
C5 C 0.5336(19) 0.5037(18) 0.2003(12) 0.016(6) Uiso 1 1 d . . .
C6 C 0.988(2) 0.221(2) 0.2151(15) 0.038(8) Uiso 1 1 d . . .
H3 H 1.0265 0.2662 0.1979 0.046 Uiso 1 1 calc R . .
C7 C 0.866(2) 0.155(2) 0.2516(13) 0.022(6) Uiso 1 1 d . . .
C8 C 0.949(2) 0.0855(19) 0.2628(15) 0.028(7) Uani 1 1 d . . .
C9 C 0.966(2) -0.016(2) 0.2876(17) 0.042(9) Uani 1 1 d . . .
C10 C 0.774(2) 0.158(2) 0.2721(13) 0.024(7) Uiso 1 1 d . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Si O1A 1.55(4) . ?
Si O1A 1.55(4) 3_666 ?
Si O1B 1.56(3) 3_666 ?
Si O1B 1.56(3) . ?
Si O2B 1.63(4) . ?
Si O2B 1.63(4) 3_666 ?
Si O2A 1.68(3) . ?
Si O2A 1.68(3) 3_666 ?
W1 O3 1.43(3) . ?
W1 O6 1.91(4) . ?
W1 O5 1.94(3) . ?
W1 O4 1.95(3) . ?
W1 O7 1.97(3) . ?
W1 O2B 2.36(4) 3_666 ?
W1 O1A 2.43(4) . ?
W2 O8 1.65(2) . ?
W2 O7 1.82(3) . ?
W2 O13 1.90(3) 3_666 ?
W2 O9 1.90(3) . ?
W2 O10 1.95(2) . ?
W2 O1A 2.38(4) . ?
W2 O1B 2.52(4) . ?
W3 O20 1.66(2) . ?
W3 O10 1.80(2) . ?
W3 O18 1.84(3) 3_666 ?
W3 O4 1.90(3) . ?
W3 O11 1.90(4) . ?
W3 O2A 2.44(4) . ?
W3 O1A 2.47(4) . ?
W4 O12 1.69(2) . ?
W4 O11 1.86(4) . ?
W4 O19 1.86(3) 3_666 ?
W4 O13 1.88(3) . ?
W4 O14 1.92(3) . ?
W4 O2A 2.29(3) . ?
W4 O1B 2.44(4) 3_666 ?
W5 O15 1.64(3) . ?
W5 O5 1.86(3) . ?
W5 O14 1.89(3) . ?
W5 O16 1.92(3) . ?
W5 O9 1.93(3) 3_666 ?
W5 O1B 2.33(3) 3_666 ?
W5 O2B 2.35(4) 3_666 ?
W6 O17 1.66(2) . ?
W6 O6 1.84(4) . ?
W6 O16 1.90(3) . ?
W6 O18 1.92(3) . ?
W6 O19 1.92(3) . ?
W6 O2A 2.36(3) 3_666 ?
W6 O2B 2.47(4) 3_666 ?
La1 O32 2.455(19) 2_655 ?
La1 O30 2.476(18) 2_655 ?
La1 O23 2.523(18) . ?
La1 O20 2.52(2) . ?
La1 O25 2.56(2) 2_645 ?
La1 O22 2.57(3) . ?
La1 O15 2.61(3) 4_565 ?
La1 N2 2.65(2) 2_645 ?
La1 O21 2.72(4) . ?
La2 O24 2.42(2) . ?
La2 O26 2.445(18) . ?
La2 O31 2.48(2) 2_755 ?
La2 O29 2.503(18) . ?
La2 O27 2.57(2) . ?
La2 N3 2.61(2) . ?
La2 O28 2.61(2) . ?
La2 O8 2.71(2) 2_645 ?
La2 O17 2.84(2) 3_666 ?
O1A O2B 1.79(5) 3_666 ?
O1A O1B 1.80(5) . ?
O1B O2B 1.75(5) . ?
O1B W5 2.33(3) 3_666 ?
O1B W4 2.44(4) 3_666 ?
O2A W6 2.36(3) 3_666 ?
O2B O1A 1.79(5) 3_666 ?
O2B W5 2.35(4) 3_666 ?
O2B W1 2.36(4) 3_666 ?
O2B W6 2.47(4) 3_666 ?
O8 La2 2.71(2) 2_655 ?
O9 W5 1.93(3) 3_666 ?
O13 W2 1.90(3) 3_666 ?
O15 La1 2.61(3) 4_566 ?
O17 La2 2.84(2) 3_666 ?
O18 W3 1.84(3) 3_666 ?
O19 W4 1.86(3) 3_666 ?
O23 C5 1.21(3) . ?
O24 C5 1.26(3) . ?
O25 C4 1.25(4) . ?
O25 La1 2.56(2) 2_655 ?
O26 C4 1.33(3) . ?
O29 C10 1.30(3) . ?
O30 C10 1.27(3) . ?
O30 La1 2.476(18) 2_645 ?
O31 C9 1.25(3) . ?
O31 La2 2.483(19) 2_745 ?
O32 C9 1.32(4) . ?
O32 La1 2.455(19) 2_645 ?
N1 C1 1.29(4) . ?
N1 C2 1.37(3) . ?
N2 C1 1.31(4) . ?
N2 C3 1.41(3) . ?
N2 La1 2.65(2) 2_655 ?
N3 C7 1.35(3) . ?
N3 C6 1.39(4) . ?
N4 C6 1.28(4) . ?
N4 C8 1.35(3) . ?
C2 C3 1.40(3) . ?
C2 C5 1.52(3) . ?
C3 C4 1.42(4) . ?
C7 C10 1.42(4) . ?
C7 C8 1.45(4) . ?
C8 C9 1.46(4) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1A Si O1A 180(2) . 3_666 ?
O1A Si O1B 109.0(19) . 3_666 ?
O1A Si O1B 71.0(19) 3_666 3_666 ?
O1A Si O1B 71.0(19) . . ?
O1A Si O1B 109.0(19) 3_666 . ?
O1B Si O1B 180(3) 3_666 . ?
O1A Si O2B 111.3(19) . . ?
O1A Si O2B 68.7(19) 3_666 . ?
O1B Si O2B 113.4(18) 3_666 . ?
O1B Si O2B 66.6(18) . . ?
O1A Si O2B 68.7(19) . 3_666 ?
O1A Si O2B 111.3(19) 3_666 3_666 ?
O1B Si O2B 66.6(18) 3_666 3_666 ?
O1B Si O2B 113.4(18) . 3_666 ?
O2B Si O2B 180.000(5) . 3_666 ?
O1A Si O2A 77.9(18) . . ?
O1A Si O2A 102.1(18) 3_666 . ?
O1B Si O2A 68.7(17) 3_666 . ?
O1B Si O2A 111.3(17) . . ?
O2B Si O2A 70.9(17) . . ?
O2B Si O2A 109.1(18) 3_666 . ?
O1A Si O2A 102.1(18) . 3_666 ?
O1A Si O2A 77.9(18) 3_666 3_666 ?
O1B Si O2A 111.3(17) 3_666 3_666 ?
O1B Si O2A 68.7(17) . 3_666 ?
O2B Si O2A 109.1(18) . 3_666 ?
O2B Si O2A 70.9(17) 3_666 3_666 ?
O2A Si O2A 180.0(14) . 3_666 ?
O3 W1 O6 99.9(15) . . ?
O3 W1 O5 97.3(11) . . ?
O6 W1 O5 83.9(14) . . ?
O3 W1 O4 100.7(13) . . ?
O6 W1 O4 159.1(14) . . ?
O5 W1 O4 90.0(11) . . ?
O3 W1 O7 102.4(12) . . ?
O6 W1 O7 91.9(15) . . ?
O5 W1 O7 160.2(13) . . ?
O4 W1 O7 87.1(12) . . ?
O3 W1 O2B 154.3(13) . 3_666 ?
O6 W1 O2B 62.9(15) . 3_666 ?
O5 W1 O2B 63.5(12) . 3_666 ?
O4 W1 O2B 96.5(12) . 3_666 ?
O7 W1 O2B 97.3(13) . 3_666 ?
O3 W1 O1A 161.8(13) . . ?
O6 W1 O1A 92.8(15) . . ?
O5 W1 O1A 97.0(12) . . ?
O4 W1 O1A 68.1(12) . . ?
O7 W1 O1A 63.8(12) . . ?
O2B W1 O1A 43.9(13) 3_666 . ?
O8 W2 O7 101.5(12) . . ?
O8 W2 O13 101.7(14) . 3_666 ?
O7 W2 O13 89.0(14) . 3_666 ?
O8 W2 O9 97.2(11) . . ?
O7 W2 O9 161.2(13) . . ?
O13 W2 O9 88.0(12) 3_666 . ?
O8 W2 O10 103.3(11) . . ?
O7 W2 O10 89.4(12) . . ?
O13 W2 O10 154.8(12) 3_666 . ?
O9 W2 O10 85.5(10) . . ?
O8 W2 O1A 162.0(12) . . ?
O7 W2 O1A 66.6(13) . . ?
O13 W2 O1A 91.9(14) 3_666 . ?
O9 W2 O1A 94.9(11) . . ?
O10 W2 O1A 64.5(11) . . ?
O8 W2 O1B 154.8(12) . . ?
O7 W2 O1B 98.7(13) . . ?
O13 W2 O1B 63.8(12) 3_666 . ?
O9 W2 O1B 63.5(11) . . ?
O10 W2 O1B 91.7(11) . . ?
O1A W2 O1B 43.0(12) . . ?
O20 W3 O10 101.2(11) . . ?
O20 W3 O18 100.8(12) . 3_666 ?
O10 W3 O18 86.2(12) . 3_666 ?
O20 W3 O4 97.3(11) . . ?
O10 W3 O4 90.3(11) . . ?
O18 W3 O4 161.9(13) 3_666 . ?
O20 W3 O11 102.4(15) . . ?
O10 W3 O11 156.3(15) . . ?
O18 W3 O11 91.4(15) 3_666 . ?
O4 W3 O11 84.7(14) . . ?
O20 W3 O2A 153.3(10) . . ?
O10 W3 O2A 98.1(11) . . ?
O18 W3 O2A 62.2(12) 3_666 . ?
O4 W3 O2A 100.8(11) . . ?
O11 W3 O2A 60.5(15) . . ?
O20 W3 O1A 157.9(11) . . ?
O10 W3 O1A 64.2(11) . . ?
O18 W3 O1A 94.9(13) 3_666 . ?
O4 W3 O1A 67.8(12) . . ?
O11 W3 O1A 92.6(15) . . ?
O2A W3 O1A 48.7(11) . . ?
O12 W4 O11 105.1(15) . . ?
O12 W4 O19 99.7(12) . 3_666 ?
O11 W4 O19 93.7(16) . 3_666 ?
O12 W4 O13 99.6(14) . . ?
O11 W4 O13 154.6(16) . . ?
O19 W4 O13 87.7(13) 3_666 . ?
O12 W4 O14 101.7(11) . . ?
O11 W4 O14 81.8(15) . . ?
O19 W4 O14 158.6(12) 3_666 . ?
O13 W4 O14 87.8(11) . . ?
O12 W4 O2A 157.5(12) . . ?
O11 W4 O2A 64.3(15) . . ?
O19 W4 O2A 63.1(12) 3_666 . ?
O13 W4 O2A 94.2(15) . . ?
O14 W4 O2A 96.4(11) . . ?
O12 W4 O1B 157.2(12) . 3_666 ?
O11 W4 O1B 89.0(15) . 3_666 ?
O19 W4 O1B 97.2(12) 3_666 3_666 ?
O13 W4 O1B 65.8(14) . 3_666 ?
O14 W4 O1B 62.0(11) . 3_666 ?
O2A W4 O1B 45.3(12) . 3_666 ?
O15 W5 O5 101.2(13) . . ?
O15 W5 O14 99.9(12) . . ?
O5 W5 O14 88.7(12) . . ?
O15 W5 O16 98.6(12) . . ?
O5 W5 O16 87.0(12) . . ?
O14 W5 O16 161.5(11) . . ?
O15 W5 O9 96.4(13) . 3_666 ?
O5 W5 O9 162.3(11) . 3_666 ?
O14 W5 O9 89.6(11) . 3_666 ?
O16 W5 O9 89.1(11) . 3_666 ?
O15 W5 O1B 156.7(14) . 3_666 ?
O5 W5 O1B 96.0(12) . 3_666 ?
O14 W5 O1B 64.7(12) . 3_666 ?
O16 W5 O1B 97.8(12) . 3_666 ?
O9 W5 O1B 67.5(12) 3_666 3_666 ?
O15 W5 O2B 159.4(14) . 3_666 ?
O5 W5 O2B 64.5(13) . 3_666 ?
O14 W5 O2B 94.7(12) . 3_666 ?
O16 W5 O2B 67.2(12) . 3_666 ?
O9 W5 O2B 98.1(12) 3_666 3_666 ?
O1B W5 O2B 43.8(12) 3_666 3_666 ?
O17 W6 O6 102.3(15) . . ?
O17 W6 O16 97.2(11) . . ?
O6 W6 O16 85.3(14) . . ?
O17 W6 O18 103.2(12) . . ?
O6 W6 O18 154.2(14) . . ?
O16 W6 O18 88.2(12) . . ?
O17 W6 O19 103.9(11) . . ?
O6 W6 O19 88.6(15) . . ?
O16 W6 O19 158.8(12) . . ?
O18 W6 O19 88.5(13) . . ?
O17 W6 O2A 158.1(12) . 3_666 ?
O6 W6 O2A 93.4(15) . 3_666 ?
O16 W6 O2A 99.2(11) . 3_666 ?
O18 W6 O2A 63.1(12) . 3_666 ?
O19 W6 O2A 60.9(12) . 3_666 ?
O17 W6 O2B 155.2(12) . 3_666 ?
O6 W6 O2B 61.2(15) . 3_666 ?
O16 W6 O2B 64.9(12) . 3_666 ?
O18 W6 O2B 93.5(12) . 3_666 ?
O19 W6 O2B 94.5(12) . 3_666 ?
O2A W6 O2B 46.6(12) 3_666 3_666 ?
O32 La1 O30 70.8(6) 2_655 2_655 ?
O32 La1 O23 143.6(6) 2_655 . ?
O30 La1 O23 73.4(6) 2_655 . ?
O32 La1 O20 78.5(7) 2_655 . ?
O30 La1 O20 72.6(6) 2_655 . ?
O23 La1 O20 84.6(6) . . ?
O32 La1 O25 73.0(7) 2_655 2_645 ?
O30 La1 O25 135.4(6) 2_655 2_645 ?
O23 La1 O25 133.1(7) . 2_645 ?
O20 La1 O25 75.4(7) . 2_645 ?
O32 La1 O22 100.3(9) 2_655 . ?
O30 La1 O22 69.9(9) 2_655 . ?
O23 La1 O22 73.3(9) . . ?
O20 La1 O22 140.5(9) . . ?
O25 La1 O22 142.7(10) 2_645 . ?
O32 La1 O15 128.8(8) 2_655 4_565 ?
O30 La1 O15 138.1(8) 2_655 4_565 ?
O23 La1 O15 83.7(8) . 4_565 ?
O20 La1 O15 140.4(7) . 4_565 ?
O25 La1 O15 85.5(8) 2_645 4_565 ?
O22 La1 O15 70.1(10) . 4_565 ?
O32 La1 N2 129.1(6) 2_655 2_645 ?
O30 La1 N2 129.9(7) 2_655 2_645 ?
O23 La1 N2 71.8(6) . 2_645 ?
O20 La1 N2 69.3(6) . 2_645 ?
O25 La1 N2 61.5(7) 2_645 2_645 ?
O22 La1 N2 129.7(9) . 2_645 ?
O15 La1 N2 71.1(7) 4_565 2_645 ?
O32 La1 O21 64.4(9) 2_655 . ?
O30 La1 O21 113.0(10) 2_655 . ?
O23 La1 O21 139.2(9) . . ?
O20 La1 O21 136.1(9) . . ?
O25 La1 O21 72.1(10) 2_645 . ?
O22 La1 O21 72.1(11) . . ?
O15 La1 O21 64.8(10) 4_565 . ?
N2 La1 O21 116.9(10) 2_645 . ?
O24 La2 O26 76.5(6) . . ?
O24 La2 O31 138.2(7) . 2_755 ?
O26 La2 O31 79.0(6) . 2_755 ?
O24 La2 O29 88.6(6) . . ?
O26 La2 O29 134.4(6) . . ?
O31 La2 O29 132.0(6) 2_755 . ?
O24 La2 O27 74.1(7) . . ?
O26 La2 O27 78.7(8) . . ?
O31 La2 O27 68.3(8) 2_755 . ?
O29 La2 O27 138.3(8) . . ?
O24 La2 N3 139.8(7) . . ?
O26 La2 N3 143.7(7) . . ?
O31 La2 N3 71.8(7) 2_755 . ?
O29 La2 N3 62.1(7) . . ?
O27 La2 N3 108.8(8) . . ?
O24 La2 O28 132.4(7) . . ?
O26 La2 O28 77.3(7) . . ?
O31 La2 O28 72.3(7) 2_755 . ?
O29 La2 O28 82.4(7) . . ?
O27 La2 O28 136.8(8) . . ?
N3 La2 O28 73.7(8) . . ?
O24 La2 O8 75.2(7) . 2_645 ?
O26 La2 O8 139.4(7) . 2_645 ?
O31 La2 O8 104.2(6) 2_755 2_645 ?
O29 La2 O8 73.1(7) . 2_645 ?
O27 La2 O8 65.9(8) . 2_645 ?
N3 La2 O8 70.4(7) . 2_645 ?
O28 La2 O8 142.9(8) . 2_645 ?
O24 La2 O17 67.4(7) . 3_666 ?
O26 La2 O17 67.8(6) . 3_666 ?
O31 La2 O17 131.0(7) 2_755 3_666 ?
O29 La2 O17 66.7(6) . 3_666 ?
O27 La2 O17 133.4(8) . 3_666 ?
N3 La2 O17 117.5(7) . 3_666 ?
O28 La2 O17 66.2(8) . 3_666 ?
O8 La2 O17 124.5(7) 2_645 3_666 ?
Si O1A O2B 57.7(17) . 3_666 ?
Si O1A O1B 54.7(17) . . ?
O2B O1A O1B 95(2) 3_666 . ?
Si O1A W2 127.4(19) . . ?
O2B O1A W2 136(2) 3_666 . ?
O1B O1A W2 72.7(17) . . ?
Si O1A W1 123.6(19) . . ?
O2B O1A W1 65.9(16) 3_666 . ?
O1B O1A W1 137(2) . . ?
W2 O1A W1 93.8(12) . . ?
Si O1A W3 118.6(18) . . ?
O2B O1A W3 125(2) 3_666 . ?
O1B O1A W3 128(2) . . ?
W2 O1A W3 92.3(13) . . ?
W1 O1A W3 91.8(12) . . ?
Si O1B O2B 58.6(16) . . ?
Si O1B O1A 54.3(16) . . ?
O2B O1B O1A 95(2) . . ?
Si O1B W5 127.3(19) . 3_666 ?
O2B O1B W5 68.8(16) . 3_666 ?
O1A O1B W5 133(2) . 3_666 ?
Si O1B W4 121.7(19) . 3_666 ?
O2B O1B W4 133(2) . 3_666 ?
O1A O1B W4 124(2) . 3_666 ?
W5 O1B W4 95.9(13) 3_666 3_666 ?
Si O1B W2 118.6(19) . . ?
O2B O1B W2 132(2) . . ?
O1A O1B W2 64.3(16) . . ?
W5 O1B W2 93.6(13) 3_666 . ?
W4 O1B W2 91.0(11) 3_666 . ?
Si O2A W4 124.4(17) . . ?
Si O2A W6 122.8(17) . 3_666 ?
W4 O2A W6 98.1(12) . 3_666 ?
Si O2A W3 114.7(16) . . ?
W4 O2A W3 95.6(12) . . ?
W6 O2A W3 94.4(12) 3_666 . ?
Si O2B O1B 54.8(16) . . ?
Si O2B O1A 53.6(16) . 3_666 ?
O1B O2B O1A 91(2) . 3_666 ?
Si O2B W5 122.0(19) . 3_666 ?
O1B O2B W5 67.3(16) . 3_666 ?
O1A O2B W5 137(2) 3_666 3_666 ?
Si O2B W1 124(2) . 3_666 ?
O1B O2B W1 133(2) . 3_666 ?
O1A O2B W1 70.1(17) 3_666 3_666 ?
W5 O2B W1 96.6(13) 3_666 3_666 ?
Si O2B W6 119.4(19) . 3_666 ?
O1B O2B W6 130(2) . 3_666 ?
O1A O2B W6 127(2) 3_666 3_666 ?
W5 O2B W6 93.7(13) 3_666 3_666 ?
W1 O2B W6 94.2(12) 3_666 3_666 ?
W3 O4 W1 132.2(15) . . ?
W5 O5 W1 135.2(16) . . ?
W6 O6 W1 142(2) . . ?
W2 O7 W1 135.4(17) . . ?
W2 O8 La2 161.7(12) . 2_655 ?
W2 O9 W5 135.0(15) . 3_666 ?
W3 O10 W2 138.0(14) . . ?
W4 O11 W3 138(2) . . ?
W4 O13 W2 139.3(18) . 3_666 ?
W5 O14 W4 136.5(15) . . ?
W5 O15 La1 157.1(14) . 4_566 ?
W6 O16 W5 134.1(15) . . ?
W6 O17 La2 177.3(14) . 3_666 ?
W3 O18 W6 140.1(17) 3_666 . ?
W4 O19 W6 137.0(16) 3_666 . ?
W3 O20 La1 155.0(11) . . ?
C5 O23 La1 171.0(18) . . ?
C5 O24 La2 152.4(18) . . ?
C4 O25 La1 124(2) . 2_655 ?
C4 O26 La2 150.0(17) . . ?
C10 O29 La2 123.9(17) . . ?
C10 O30 La1 155.6(17) . 2_645 ?
C9 O31 La2 160(2) . 2_745 ?
C9 O32 La1 157.0(18) . 2_645 ?
C1 N1 C2 108(2) . . ?
C1 N2 C3 102(2) . . ?
C1 N2 La1 140(2) . 2_655 ?
C3 N2 La1 118.5(15) . 2_655 ?
C7 N3 C6 105(2) . . ?
C7 N3 La2 118.4(16) . . ?
C6 N3 La2 134.7(19) . . ?
C6 N4 C8 113(3) . . ?
N1 C1 N2 116(3) . . ?
N1 C2 C3 104(2) . . ?
N1 C2 C5 116(2) . . ?
C3 C2 C5 140(2) . . ?
C2 C3 N2 110(2) . . ?
C2 C3 C4 136(2) . . ?
N2 C3 C4 114(2) . . ?
O25 C4 O26 116(3) . . ?
O25 C4 C3 122(3) . . ?
O26 C4 C3 122(3) . . ?
O23 C5 O24 127(2) . . ?
O23 C5 C2 116(2) . . ?
O24 C5 C2 117(2) . . ?
N4 C6 N3 110(3) . . ?
N3 C7 C10 117(2) . . ?
N3 C7 C8 110(2) . . ?
C10 C7 C8 132(3) . . ?
N4 C8 C7 102(2) . . ?
N4 C8 C9 122(3) . . ?
C7 C8 C9 135(3) . . ?
O31 C9 O32 123(3) . . ?
O31 C9 C8 115(3) . . ?
O32 C9 C8 121(3) . . ?
O30 C10 O29 119(2) . . ?
O30 C10 C7 123(3) . . ?
O29 C10 C7 118(2) . . ?

_diffrn_measured_fraction_theta_max 0.987
_diffrn_reflns_theta_full        25.75
_diffrn_measured_fraction_theta_full 0.987
_refine_diff_density_max         2.896
_refine_diff_density_min         -3.600
_refine_diff_density_rms         0.494
_database_code_depnum_ccdc_archive 'CCDC 936028'
#######################################################################
#
#                 Cambridge Crystallographic Data Centre
#                                CCDC 
# 
#######################################################################
# 
#  This CIF contains data from an original supplementary publication
#  deposited with the CCDC, and may include chemical, crystal,
#  experimental, refinement, atomic coordinates,
#  anisotropic displacement parameters and molecular geometry data,
#  as required by the journal to which it was submitted.
#
#  This CIF is provided on the understanding that it is used for bona
#  fide research purposes only. It may contain copyright material
#  of the CCDC or of third parties, and may not be copied or further
#  disseminated in any form, whether machine-readable or not,
#  except for the purpose of generating routine backup copies
#  on your local computer system.
# 
#  For further information on the CCDC, data deposition and
#  data retrieval see:
#                         www.ccdc.cam.ac.uk
#
#  Bona fide researchers may freely download Mercury and enCIFer
#  from this site to visualise CIF-encoded structures and 
#  to carry out CIF format checking respectively.
#
data_4

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
;
 ?
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         C20H46Ce4N8O75SiW12
_chemical_formula_sum            'C20 H46 Ce4 N8 O75 Si W12'
_chemical_formula_weight         4393.22

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ce Ce -0.2486 2.6331 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_H-M   'p 21/c'
_symmetry_space_group_name_Hall  '-p 2ybc'

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'

_cell_length_a                   13.7014(10)
_cell_length_b                   13.1554(10)
_cell_length_c                   22.7273(17)
_cell_angle_alpha                90.00
_cell_angle_beta                 100.3660(10)
_cell_angle_gamma                90.00
_cell_volume                     4029.7(5)
_cell_formula_units_Z            2
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    .
_cell_measurement_theta_min      .
_cell_measurement_theta_max      .

_exptl_crystal_description       block
_exptl_crystal_colour            yellow
_exptl_crystal_size_max          0.09
_exptl_crystal_size_mid          0.07
_exptl_crystal_size_min          0.05
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    3.620
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             3884
_exptl_absorpt_coefficient_mu    19.398
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.209
_exptl_absorpt_correction_T_max  0.385
_exptl_absorpt_process_details   'SADABS (Sheldrick, 2001)'

_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_detector_area_resol_mean .
_diffrn_standards_number         .
_diffrn_standards_interval_count .
_diffrn_standards_interval_time  .
_diffrn_standards_decay_%        .
_diffrn_reflns_number            21194
_diffrn_reflns_av_R_equivalents  0.0344
_diffrn_reflns_av_sigmaI/netI    0.0414
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_l_min       -28
_diffrn_reflns_limit_l_max       27
_diffrn_reflns_theta_min         2.16
_diffrn_reflns_theta_max         26.00
_reflns_number_total             7821
_reflns_number_gt                7265
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       'SMART (Bruker, 2007)'
_computing_cell_refinement       'SMART (Bruker, 2007)'
_computing_data_reduction        'SMART (Bruker, 2007)'
_computing_structure_solution    'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    'SHELXL-97 (Sheldrick, 1997)'
_computing_publication_material  'SHELXL-97 (Sheldrick, 1997)'

_refine_special_details          
;
 Refinement of F² against ALL reflections.  The weighted R-factor wR and
 goodness of fit S are based on F², conventional R-factors R are based
 on F, with F set to zero for negative F². The threshold expression of
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is
 not relevant to the choice of reflections for refinement.  R-factors based
 on F² are statistically about twice as large as those based on F, and R-
 factors based on ALL data will be even larger.
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0001P)²+825.1682P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_number_reflns         7821
_refine_ls_number_parameters     438
_refine_ls_number_restraints     6
_refine_ls_R_factor_all          0.0782
_refine_ls_R_factor_gt           0.0730
_refine_ls_wR_factor_ref         0.1514
_refine_ls_wR_factor_gt          0.1487
_refine_ls_goodness_of_fit_ref   1.014
_refine_ls_restrained_S_all      1.069
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Si Si 0.5000 0.5000 0.5000 0.0098(15) Uani 1 2 d S . .
W1 W 0.61763(7) 0.30098(6) 0.43764(4) 0.01338(19) Uani 1 1 d . . .
W2 W 0.49000(7) 0.25201(7) 0.55738(4) 0.0200(2) Uani 1 1 d . . .
W3 W 0.35508(7) 0.31079(7) 0.41311(4) 0.0179(2) Uani 1 1 d . . .
W4 W 0.36792(8) 0.55863(8) 0.35785(4) 0.0239(2) Uani 1 1 d U . .
W5 W 0.62935(7) 0.54855(8) 0.38009(4) 0.0214(2) Uani 1 1 d . . .
W6 W 0.76181(7) 0.48805(8) 0.52395(5) 0.0252(2) Uani 1 1 d . . .
Ce1 Ce 0.21878(8) 0.10085(8) 0.27619(5) 0.0090(2) Uani 1 1 d . . .
Ce2 Ce 0.27607(8) 0.60101(8) 0.17853(5) 0.0067(2) Uani 1 1 d . . .
O1A O 0.4976(18) 0.3856(19) 0.4808(11) 0.004(5) Uiso 0.50 1 d P . .
O1B O 0.596(2) 0.465(2) 0.4720(12) 0.009(5) Uiso 0.50 1 d P . .
O2A O 0.5052(19) 0.570(2) 0.4395(12) 0.006(5) Uiso 0.50 1 d P . .
O2B O 0.395(2) 0.473(2) 0.4534(13) 0.012(6) Uiso 0.50 1 d P . .
O3 O 0.6682(17) 0.2012(17) 0.4052(8) 0.046(6) Uani 1 1 d . . .
O4 O 0.4840(16) 0.2814(17) 0.4018(10) 0.044(5) Uiso 1 1 d . . .
O5 O 0.6268(18) 0.4062(19) 0.3833(11) 0.053(6) Uiso 1 1 d . . .
O6 O 0.7284(19) 0.358(2) 0.4871(11) 0.057(6) Uiso 1 1 d . . .
O7 O 0.5853(14) 0.235(2) 0.5055(9) 0.050(7) Uani 1 1 d . . .
O8 O 0.4870(14) 0.1332(15) 0.5845(9) 0.037(5) Uani 1 1 d . . .
O9 O 0.3884(15) 0.244(2) 0.4876(9) 0.055(7) Uani 1 1 d . . .
O10 O 0.3565(18) 0.4180(18) 0.3578(11) 0.050(6) Uiso 1 1 d . . .
O11 O 0.2552(19) 0.564(2) 0.3986(11) 0.057(6) Uiso 1 1 d . . .
O12 O 0.406(2) 0.684(2) 0.3914(12) 0.064(7) Uiso 1 1 d . . .
O13 O 0.4952(15) 0.5415(19) 0.3424(14) 0.077(10) Uani 1 1 d . . .
O14 O 0.6887(12) 0.5704(13) 0.3228(8) 0.023(4) Uiso 1 1 d . . .
O15 O 0.604(2) 0.683(2) 0.4024(14) 0.079(9) Uiso 1 1 d . . .
O16 O 0.7310(19) 0.546(2) 0.4475(12) 0.057(6) Uiso 1 1 d . . .
O17 O 0.8821(19) 0.4811(16) 0.5333(11) 0.051(6) Uani 1 1 d . . .
O18 O 0.753(2) 0.623(2) 0.5568(12) 0.065(7) Uiso 1 1 d . . .
O19 O 0.2891(14) 0.2199(15) 0.3694(8) 0.032(4) Uani 1 1 d . . .
O20 O 0.3008(13) 0.5877(13) 0.2889(7) 0.024(4) Uani 1 1 d . . .
O21 O 0.2271(15) 0.0109(16) 0.3760(8) 0.035(5) Uani 1 1 d . . .
O22 O 0.1004(14) 0.0952(18) 0.1762(10) 0.045(6) Uani 1 1 d . . .
O23 O 0.2763(11) 0.2595(12) 0.2362(7) 0.018(3) Uani 1 1 d . . .
O24 O 0.2655(10) 0.4178(11) 0.2061(7) 0.013(3) Uani 1 1 d . . .
O25 O 0.1078(11) 0.5663(12) 0.1990(8) 0.020(3) Uani 1 1 d . . .
O26 O -0.0517(11) 0.5473(12) 0.2051(8) 0.023(4) Uani 1 1 d . . .
O27 O 0.283(2) 0.487(2) 0.0860(10) 0.071(9) Uani 1 1 d . . .
O28 O 0.136(2) 0.661(2) 0.0946(14) 0.080(9) Uiso 1 1 d . . .
O29 O 0.2090(13) 0.7677(12) 0.2104(8) 0.027(4) Uani 1 1 d . . .
O30 O 0.2170(11) 0.9222(11) 0.2482(8) 0.019(3) Uani 1 1 d . . .
O31 O 0.5514(10) 1.0282(11) 0.3113(7) 0.013(3) Uani 1 1 d . . .
O32 O 0.3905(11) 1.0507(11) 0.3052(7) 0.014(3) Uiso 1 1 d . . .
O33 O 0.096(2) 0.660(2) 0.3262(12) 0.066(8) Uani 1 1 d . . .
O34 O 0.214(2) 0.806(2) 0.3896(17) 0.091(11) Uani 1 1 d . . .
O35 O -0.066(3) 0.602(4) 0.070(2) 0.128(15) Uiso 1 1 d . . .
O36 O 0.189(5) 0.299(6) 0.050(5) 0.18(6) Uani 0.50 1 d P . .
O37 O 0.056(7) 0.206(7) 0.045(4) 0.13(3) Uiso 0.50 1 d P . .
O38 O 0.086(3) -0.084(3) 0.1028(13) 0.091(10) Uani 1 1 d . . .
O39 O 0.4971(17) -0.0602(14) 0.5692(7) 0.035(5) Uani 1 1 d . . .
O40 O 0.628(4) -0.003(4) 0.527(2) 0.140(17) Uiso 1 1 d . . .
N1 N 0.1077(14) 0.2600(15) 0.2766(9) 0.018(4) Uiso 1 1 d . . .
N2 N -0.0153(14) 0.3696(15) 0.2646(9) 0.019(4) Uiso 1 1 d . . .
H4 H -0.0725 0.3956 0.2659 0.023 Uiso 1 1 calc R . .
N3 N 0.5309(13) 0.8379(13) 0.2665(8) 0.012(4) Uiso 1 1 d . . .
H2 H 0.5915 0.8555 0.2791 0.015 Uiso 1 1 calc R . .
N4 N 0.4036(13) 0.7434(13) 0.2268(8) 0.012(3) Uiso 1 1 d . . .
C1 C 0.0151(17) 0.2789(17) 0.2851(11) 0.019(5) Uani 1 1 d . . .
H3 H -0.0228 0.2339 0.3031 0.023 Uiso 1 1 calc R . .
C2 C 0.1329(15) 0.3461(16) 0.2475(9) 0.012(4) Uani 1 1 d . . .
C3 C 0.0564(15) 0.4143(16) 0.2418(9) 0.012(4) Uiso 1 1 d . . .
C4 C 0.0371(15) 0.5181(15) 0.2123(9) 0.010(4) Uani 1 1 d . . .
C5 C 0.2304(15) 0.3431(16) 0.2288(9) 0.012(4) Uiso 1 1 d . . .
C6 C 0.4999(15) 0.7512(18) 0.2399(10) 0.017(5) Uani 1 1 d . . .
H1 H 0.5427 0.7007 0.2314 0.020 Uiso 1 1 calc R . .
C7 C 0.4457(13) 0.8953(14) 0.2702(8) 0.006(4) Uiso 1 1 d . . .
C8 C 0.3680(14) 0.8344(15) 0.2470(8) 0.007(4) Uiso 1 1 d . . .
C9 C 0.2590(15) 0.8391(16) 0.2343(9) 0.012(4) Uiso 1 1 d . . .
C10 C 0.4651(14) 1.0001(15) 0.2971(9) 0.009(4) Uiso 1 1 d . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Si O1A 1.57(3) . ?
Si O1A 1.57(3) 3_666 ?
Si O1B 1.63(3) 3_666 ?
Si O1B 1.63(3) . ?
Si O2A 1.67(3) . ?
Si O2A 1.67(3) 3_666 ?
Si O2B 1.66(3) 3_666 ?
Si O2B 1.66(3) . ?
W1 O3 1.713(17) . ?
W1 O5 1.87(2) . ?
W1 O6 1.87(3) . ?
W1 O4 1.88(2) . ?
W1 O7 1.891(19) . ?
W1 O1B 2.33(3) . ?
W1 O1A 2.34(2) . ?
W2 O8 1.683(18) . ?
W2 O12 1.88(3) 3_666 ?
W2 O15 1.91(3) 3_666 ?
W2 O9 1.92(2) . ?
W2 O7 1.92(2) . ?
W2 O2A 2.35(3) 3_666 ?
W2 O1A 2.49(2) . ?
W3 O19 1.707(18) . ?
W3 O4 1.87(2) . ?
W3 O9 1.89(2) . ?
W3 O10 1.89(2) . ?
W3 O18 1.94(3) 3_666 ?
W3 O2B 2.35(3) . ?
W3 O1A 2.46(3) . ?
W4 O20 1.711(16) . ?
W4 O12 1.84(3) . ?
W4 O13 1.85(2) . ?
W4 O10 1.86(2) . ?
W4 O11 1.94(3) . ?
W4 O2A 2.40(3) . ?
W4 O2B 2.41(3) . ?
W5 O14 1.680(17) . ?
W5 O5 1.87(2) . ?
W5 O16 1.88(3) . ?
W5 O13 1.88(2) . ?
W5 O15 1.89(3) . ?
W5 O2A 2.37(3) . ?
W5 O1B 2.47(3) . ?
W6 O17 1.63(3) . ?
W6 O16 1.87(3) . ?
W6 O6 1.93(3) . ?
W6 O11 1.94(3) 3_666 ?
W6 O18 1.94(3) . ?
W6 O2B 2.35(3) 3_666 ?
W6 O1B 2.38(3) . ?
Ce1 O32 2.418(15) 1_545 ?
Ce1 O30 2.433(14) 1_545 ?
Ce1 O23 2.462(16) . ?
Ce1 O26 2.504(16) 2_545 ?
Ce1 O21 2.542(18) . ?
Ce1 O22 2.545(19) . ?
Ce1 N1 2.589(19) . ?
Ce1 O19 2.670(18) . ?
Ce1 O14 2.802(17) 2_645 ?
Ce2 O25 2.475(15) . ?
Ce2 O20 2.476(16) . ?
Ce2 O24 2.500(14) . ?
Ce2 O31 2.522(14) 2_645 ?
Ce2 O29 2.534(16) . ?
Ce2 O3 2.542(17) 2_655 ?
Ce2 O28 2.57(3) . ?
Ce2 O27 2.60(2) . ?
Ce2 N4 2.660(18) . ?
O1A O1B 1.75(4) . ?
O2A W2 2.35(3) 3_666 ?
O2B W6 2.35(3) 3_666 ?
O3 Ce2 2.542(17) 2_645 ?
O11 W6 1.94(3) 3_666 ?
O12 W2 1.88(3) 3_666 ?
O14 Ce1 2.802(17) 2_655 ?
O15 W2 1.91(3) 3_666 ?
O18 W3 1.94(3) 3_666 ?
O23 C5 1.26(3) . ?
O24 C5 1.25(2) . ?
O25 C4 1.24(3) . ?
O26 C4 1.26(3) . ?
O26 Ce1 2.504(16) 2 ?
O29 C9 1.23(3) . ?
O30 C9 1.30(3) . ?
O30 Ce1 2.433(14) 1_565 ?
O31 C10 1.23(2) . ?
O31 Ce2 2.522(14) 2_655 ?
O32 C10 1.26(2) . ?
O32 Ce1 2.418(15) 1_565 ?
N1 C1 1.34(3) . ?
N1 C2 1.39(3) . ?
N2 C1 1.32(3) . ?
N2 C3 1.33(3) . ?
N3 C6 1.32(3) . ?
N3 C7 1.41(2) . ?
N4 C6 1.30(3) . ?
N4 C8 1.40(3) . ?
C2 C3 1.37(3) . ?
C2 C5 1.47(3) . ?
C3 C4 1.52(3) . ?
C7 C8 1.36(3) . ?
C7 C10 1.51(3) . ?
C8 C9 1.47(3) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1A Si O1A 180.0(18) . 3_666 ?
O1A Si O1B 113.8(13) . 3_666 ?
O1A Si O1B 66.2(13) 3_666 3_666 ?
O1A Si O1B 66.2(13) . . ?
O1A Si O1B 113.8(13) 3_666 . ?
O1B Si O1B 180.0(16) 3_666 . ?
O1A Si O2A 107.6(13) . . ?
O1A Si O2A 72.4(13) 3_666 . ?
O1B Si O2A 108.9(13) 3_666 . ?
O1B Si O2A 71.1(13) . . ?
O1A Si O2A 72.4(13) . 3_666 ?
O1A Si O2A 107.6(13) 3_666 3_666 ?
O1B Si O2A 71.1(13) 3_666 3_666 ?
O1B Si O2A 108.9(13) . 3_666 ?
O2A Si O2A 180.000(6) . 3_666 ?
O1A Si O2B 110.6(14) . 3_666 ?
O1A Si O2B 69.4(14) 3_666 3_666 ?
O1B Si O2B 111.1(14) 3_666 3_666 ?
O1B Si O2B 68.9(14) . 3_666 ?
O2A Si O2B 104.5(13) . 3_666 ?
O2A Si O2B 75.5(13) 3_666 3_666 ?
O1A Si O2B 69.4(14) . . ?
O1A Si O2B 110.6(13) 3_666 . ?
O1B Si O2B 68.9(14) 3_666 . ?
O1B Si O2B 111.1(14) . . ?
O2A Si O2B 75.5(13) . . ?
O2A Si O2B 104.5(13) 3_666 . ?
O2B Si O2B 180.000(5) 3_666 . ?
O3 W1 O5 101.7(11) . . ?
O3 W1 O6 102.6(11) . . ?
O5 W1 O6 87.6(11) . . ?
O3 W1 O4 98.4(10) . . ?
O5 W1 O4 89.5(10) . . ?
O6 W1 O4 159.0(10) . . ?
O3 W1 O7 99.9(11) . . ?
O5 W1 O7 158.4(11) . . ?
O6 W1 O7 88.7(10) . . ?
O4 W1 O7 86.4(9) . . ?
O3 W1 O1B 159.9(11) . . ?
O5 W1 O1B 64.2(10) . . ?
O6 W1 O1B 64.4(10) . . ?
O4 W1 O1B 95.8(9) . . ?
O7 W1 O1B 95.1(11) . . ?
O3 W1 O1A 156.1(11) . . ?
O5 W1 O1A 93.5(10) . . ?
O6 W1 O1A 96.5(10) . . ?
O4 W1 O1A 63.0(9) . . ?
O7 W1 O1A 65.9(10) . . ?
O1B W1 O1A 43.9(9) . . ?
O8 W2 O12 105.0(11) . 3_666 ?
O8 W2 O15 100.3(12) . 3_666 ?
O12 W2 O15 90.3(13) 3_666 3_666 ?
O8 W2 O9 101.0(11) . . ?
O12 W2 O9 153.8(12) 3_666 . ?
O15 W2 O9 88.2(12) 3_666 . ?
O8 W2 O7 100.4(10) . . ?
O12 W2 O7 84.7(11) 3_666 . ?
O15 W2 O7 159.4(13) 3_666 . ?
O9 W2 O7 87.6(9) . . ?
O8 W2 O2A 156.8(10) . 3_666 ?
O12 W2 O2A 61.0(11) 3_666 3_666 ?
O15 W2 O2A 63.6(12) 3_666 3_666 ?
O9 W2 O2A 95.2(11) . 3_666 ?
O7 W2 O2A 96.7(10) . 3_666 ?
O8 W2 O1A 156.7(10) . . ?
O12 W2 O1A 89.5(10) 3_666 . ?
O15 W2 O1A 97.7(11) 3_666 . ?
O9 W2 O1A 64.8(9) . . ?
O7 W2 O1A 62.3(9) . . ?
O2A W2 O1A 46.4(9) 3_666 . ?
O19 W3 O4 100.9(10) . . ?
O19 W3 O9 102.4(11) . . ?
O4 W3 O9 86.9(9) . . ?
O19 W3 O10 101.7(10) . . ?
O4 W3 O10 86.6(10) . . ?
O9 W3 O10 155.8(11) . . ?
O19 W3 O18 99.4(11) . 3_666 ?
O4 W3 O18 159.7(11) . 3_666 ?
O9 W3 O18 88.2(11) . 3_666 ?
O10 W3 O18 90.0(11) . 3_666 ?
O19 W3 O2B 157.8(10) . . ?
O4 W3 O2B 94.8(10) . . ?
O9 W3 O2B 94.1(11) . . ?
O10 W3 O2B 63.3(10) . . ?
O18 W3 O2B 66.0(11) 3_666 . ?
O19 W3 O1A 157.1(9) . . ?
O4 W3 O1A 60.5(9) . . ?
O9 W3 O1A 65.7(9) . . ?
O10 W3 O1A 90.9(9) . . ?
O18 W3 O1A 99.7(10) 3_666 . ?
O2B W3 O1A 44.9(9) . . ?
O20 W4 O12 104.1(10) . . ?
O20 W4 O13 102.8(12) . . ?
O12 W4 O13 89.1(11) . . ?
O20 W4 O10 101.0(10) . . ?
O12 W4 O10 154.8(12) . . ?
O13 W4 O10 87.8(11) . . ?
O20 W4 O11 95.0(10) . . ?
O12 W4 O11 87.7(11) . . ?
O13 W4 O11 162.2(13) . . ?
O10 W4 O11 87.8(11) . . ?
O20 W4 O2A 155.9(9) . . ?
O12 W4 O2A 60.2(11) . . ?
O13 W4 O2A 61.4(11) . . ?
O10 W4 O2A 96.7(10) . . ?
O11 W4 O2A 102.1(10) . . ?
O20 W4 O2B 153.9(9) . . ?
O12 W4 O2B 93.2(11) . . ?
O13 W4 O2B 96.7(13) . . ?
O10 W4 O2B 62.4(10) . . ?
O11 W4 O2B 66.0(10) . . ?
O2A W4 O2B 50.2(9) . . ?
O14 W5 O5 102.5(9) . . ?
O14 W5 O16 104.2(10) . . ?
O5 W5 O16 87.9(11) . . ?
O14 W5 O13 103.0(12) . . ?
O5 W5 O13 86.9(11) . . ?
O16 W5 O13 152.9(13) . . ?
O14 W5 O15 100.7(11) . . ?
O5 W5 O15 156.8(12) . . ?
O16 W5 O15 86.9(13) . . ?
O13 W5 O15 87.5(12) . . ?
O14 W5 O2A 156.7(9) . . ?
O5 W5 O2A 94.3(10) . . ?
O16 W5 O2A 92.3(10) . . ?
O13 W5 O2A 61.6(11) . . ?
O15 W5 O2A 63.4(11) . . ?
O14 W5 O1B 156.7(8) . . ?
O5 W5 O1B 61.0(10) . . ?
O16 W5 O1B 61.5(10) . . ?
O13 W5 O1B 92.9(13) . . ?
O15 W5 O1B 96.8(11) . . ?
O2A W5 O1B 46.5(9) . . ?
O17 W6 O16 101.4(12) . . ?
O17 W6 O6 99.4(11) . . ?
O16 W6 O6 87.7(11) . . ?
O17 W6 O11 98.4(11) . 3_666 ?
O16 W6 O11 160.1(11) . 3_666 ?
O6 W6 O11 91.4(11) . 3_666 ?
O17 W6 O18 97.8(11) . . ?
O16 W6 O18 88.1(11) . . ?
O6 W6 O18 162.8(11) . . ?
O11 W6 O18 86.9(11) 3_666 . ?
O17 W6 O2B 158.0(11) . 3_666 ?
O16 W6 O2B 93.1(10) . 3_666 ?
O6 W6 O2B 97.6(10) . 3_666 ?
O11 W6 O2B 67.3(10) 3_666 3_666 ?
O18 W6 O2B 66.0(11) . 3_666 ?
O17 W6 O1B 155.6(10) . . ?
O16 W6 O1B 63.6(10) . . ?
O6 W6 O1B 62.6(10) . . ?
O11 W6 O1B 98.4(10) 3_666 . ?
O18 W6 O1B 100.7(10) . . ?
O2B W6 O1B 46.4(9) 3_666 . ?
O32 Ce1 O30 76.8(5) 1_545 1_545 ?
O32 Ce1 O23 88.4(5) 1_545 . ?
O30 Ce1 O23 135.3(5) 1_545 . ?
O32 Ce1 O26 138.7(5) 1_545 2_545 ?
O30 Ce1 O26 78.8(5) 1_545 2_545 ?
O23 Ce1 O26 131.7(5) . 2_545 ?
O32 Ce1 O21 75.2(6) 1_545 . ?
O30 Ce1 O21 77.3(6) 1_545 . ?
O23 Ce1 O21 139.3(6) . . ?
O26 Ce1 O21 67.2(6) 2_545 . ?
O32 Ce1 O22 131.9(6) 1_545 . ?
O30 Ce1 O22 76.3(7) 1_545 . ?
O23 Ce1 O22 83.7(7) . . ?
O26 Ce1 O22 71.9(7) 2_545 . ?
O21 Ce1 O22 134.6(7) . . ?
O32 Ce1 N1 139.8(6) 1_545 . ?
O30 Ce1 N1 143.5(6) 1_545 . ?
O23 Ce1 N1 62.9(5) . . ?
O26 Ce1 N1 70.8(6) 2_545 . ?
O21 Ce1 N1 107.7(6) . . ?
O22 Ce1 N1 75.3(7) . . ?
O32 Ce1 O19 75.5(6) 1_545 . ?
O30 Ce1 O19 139.3(6) 1_545 . ?
O23 Ce1 O19 72.6(5) . . ?
O26 Ce1 O19 103.9(5) 2_545 . ?
O21 Ce1 O19 67.3(6) . . ?
O22 Ce1 O19 143.8(7) . . ?
N1 Ce1 O19 69.6(6) . . ?
O32 Ce1 O14 67.8(5) 1_545 2_645 ?
O30 Ce1 O14 68.7(5) 1_545 2_645 ?
O23 Ce1 O14 66.7(5) . 2_645 ?
O26 Ce1 O14 131.0(5) 2_545 2_645 ?
O21 Ce1 O14 134.1(6) . 2_645 ?
O22 Ce1 O14 65.6(6) . 2_645 ?
N1 Ce1 O14 118.0(5) . 2_645 ?
O19 Ce1 O14 124.7(5) . 2_645 ?
O25 Ce2 O20 76.1(6) . . ?
O25 Ce2 O24 71.2(5) . . ?
O20 Ce2 O24 71.4(5) . . ?
O25 Ce2 O31 143.3(5) . 2_645 ?
O20 Ce2 O31 85.7(5) . 2_645 ?
O24 Ce2 O31 72.9(5) . 2_645 ?
O25 Ce2 O29 73.0(5) . . ?
O20 Ce2 O29 76.2(6) . . ?
O24 Ce2 O29 136.2(5) . . ?
O31 Ce2 O29 133.2(5) 2_645 . ?
O25 Ce2 O3 130.7(7) . 2_655 ?
O20 Ce2 O3 142.2(6) . 2_655 ?
O24 Ce2 O3 136.5(6) . 2_655 ?
O31 Ce2 O3 82.1(7) 2_645 2_655 ?
O29 Ce2 O3 86.5(7) . 2_655 ?
O25 Ce2 O28 66.5(8) . . ?
O20 Ce2 O28 136.1(8) . . ?
O24 Ce2 O28 114.3(8) . . ?
O31 Ce2 O28 138.2(8) 2_645 . ?
O29 Ce2 O28 71.7(8) . . ?
O3 Ce2 O28 64.5(9) 2_655 . ?
O25 Ce2 O27 102.6(8) . . ?
O20 Ce2 O27 139.6(7) . . ?
O24 Ce2 O27 70.2(7) . . ?
O31 Ce2 O27 71.6(8) 2_645 . ?
O29 Ce2 O27 143.0(8) . . ?
O3 Ce2 O27 68.4(8) 2_655 . ?
O28 Ce2 O27 73.0(10) . . ?
O25 Ce2 N4 128.1(5) . . ?
O20 Ce2 N4 70.9(6) . . ?
O24 Ce2 N4 129.7(5) . . ?
O31 Ce2 N4 72.2(5) 2_645 . ?
O29 Ce2 N4 61.2(5) . . ?
O3 Ce2 N4 71.3(6) 2_655 . ?
O28 Ce2 N4 115.9(8) . . ?
O27 Ce2 N4 128.4(8) . . ?
Si O1A O1B 58.6(12) . . ?
Si O1A W1 126.3(13) . . ?
O1B O1A W1 67.7(12) . . ?
Si O1A W3 122.2(13) . . ?
O1B O1A W3 135.2(16) . . ?
W1 O1A W3 94.9(9) . . ?
Si O1A W2 119.1(13) . . ?
O1B O1A W2 129.3(15) . . ?
W1 O1A W2 94.5(9) . . ?
W3 O1A W2 91.5(8) . . ?
Si O1B O1A 55.1(12) . . ?
Si O1B W1 123.5(14) . . ?
O1A O1B W1 68.4(12) . . ?
Si O1B W6 122.4(14) . . ?
O1A O1B W6 135.0(16) . . ?
W1 O1B W6 96.8(10) . . ?
Si O1B W5 119.2(14) . . ?
O1A O1B W5 128.7(16) . . ?
W1 O1B W5 94.3(9) . . ?
W6 O1B W5 93.3(9) . . ?
Si O2A W2 122.1(13) . 3_666 ?
Si O2A W5 123.1(13) . . ?
W2 O2A W5 96.6(9) 3_666 . ?
Si O2A W4 117.5(13) . . ?
W2 O2A W4 95.7(9) 3_666 . ?
W5 O2A W4 95.5(9) . . ?
Si O2B W3 123.5(15) . . ?
Si O2B W6 122.3(15) . 3_666 ?
W3 O2B W6 97.1(10) . 3_666 ?
Si O2B W4 116.8(14) . . ?
W3 O2B W4 94.9(10) . . ?
W6 O2B W4 95.7(10) 3_666 . ?
W1 O3 Ce2 156.8(11) . 2_645 ?
W3 O4 W1 141.3(13) . . ?
W1 O5 W5 140.2(14) . . ?
W1 O6 W6 136.0(14) . . ?
W1 O7 W2 137.0(14) . . ?
W3 O9 W2 137.7(13) . . ?
W4 O10 W3 138.9(14) . . ?
W4 O11 W6 131.0(14) . 3_666 ?
W4 O12 W2 141.6(16) . 3_666 ?
W4 O13 W5 141.4(17) . . ?
W5 O14 Ce1 177.3(9) . 2_655 ?
W5 O15 W2 136.1(18) . 3_666 ?
W6 O16 W5 140.9(15) . . ?
W3 O18 W6 130.7(15) 3_666 . ?
W3 O19 Ce1 161.9(10) . . ?
W4 O20 Ce2 153.7(10) . . ?
C5 O23 Ce1 127.0(13) . . ?
C5 O24 Ce2 155.2(13) . . ?
C4 O25 Ce2 159.2(14) . . ?
C4 O26 Ce1 162.9(16) . 2 ?
C9 O29 Ce2 125.8(14) . . ?
C9 O30 Ce1 153.0(13) . 1_565 ?
C10 O31 Ce2 169.3(14) . 2_655 ?
C10 O32 Ce1 151.5(14) . 1_565 ?
C1 N1 C2 103.9(18) . . ?
C1 N1 Ce1 136.3(15) . . ?
C2 N1 Ce1 117.5(13) . . ?
C1 N2 C3 109.2(19) . . ?
C6 N3 C7 106.7(17) . . ?
C6 N4 C8 104.8(17) . . ?
C6 N4 Ce2 135.4(15) . . ?
C8 N4 Ce2 119.7(12) . . ?
N2 C1 N1 111.4(19) . . ?
C3 C2 N1 109.2(18) . . ?
C3 C2 C5 135(2) . . ?
N1 C2 C5 115.6(18) . . ?
N2 C3 C2 106.3(19) . . ?
N2 C3 C4 119.1(19) . . ?
C2 C3 C4 134.4(19) . . ?
O25 C4 O26 126.2(19) . . ?
O25 C4 C3 119.0(18) . . ?
O26 C4 C3 114.8(18) . . ?
O24 C5 O23 121.4(19) . . ?
O24 C5 C2 122.4(19) . . ?
O23 C5 C2 116.1(18) . . ?
N4 C6 N3 114(2) . . ?
C8 C7 N3 105.1(16) . . ?
C8 C7 C10 139.6(18) . . ?
N3 C7 C10 115.3(16) . . ?
C7 C8 N4 109.6(16) . . ?
C7 C8 C9 138.4(18) . . ?
N4 C8 C9 111.9(17) . . ?
O29 C9 O30 120.8(19) . . ?
O29 C9 C8 121.4(19) . . ?
O30 C9 C8 117.7(18) . . ?
O31 C10 O32 124.9(19) . . ?
O31 C10 C7 118.1(17) . . ?
O32 C10 C7 116.9(17) . . ?

_diffrn_measured_fraction_theta_max 0.988
_diffrn_reflns_theta_full        26.00
_diffrn_measured_fraction_theta_full 0.988
_refine_diff_density_max         5.024
_refine_diff_density_min         -3.628
_refine_diff_density_rms         0.476
_database_code_depnum_ccdc_archive 'CCDC 936029'
